# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_120

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            ' Gd  Ge3   H2   K3 O10'
_chemical_formula_weight         654.34

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnma

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, y+1/2, -z'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'-x-1/2, y-1/2, z-1/2'
'x, -y-1/2, z'

_cell_length_a                   13.6880(7)
_cell_length_b                   13.6891(7)
_cell_length_c                   6.0821(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     1139.64(10)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    4096
_cell_measurement_theta_min      5.965
_cell_measurement_theta_max      62.182

_exptl_crystal_description       rod
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.814
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1196
_exptl_absorpt_coefficient_mu    14.712
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.498
_exptl_absorpt_correction_T_max  0.555
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            6064
_diffrn_reflns_av_R_equivalents  0.0207
_diffrn_reflns_av_sigmaI/netI    0.0170
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_theta_min         2.98
_diffrn_reflns_theta_max         26.35
_reflns_number_total             1213
_reflns_number_gt                1138
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         1213
_refine_ls_number_parameters     85
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0193
_refine_ls_R_factor_gt           0.0181
_refine_ls_wR_factor_ref         0.0798
_refine_ls_wR_factor_gt          0.0774
_refine_ls_goodness_of_fit_ref   0.721
_refine_ls_restrained_S_all      0.721
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Gd1 Gd 0.458165(16) 0.2500 0.91224(3) 0.00698(15) Uani 1 2 d S . .
Ge1 Ge 0.40083(3) 0.09972(3) 0.40898(5) 0.00912(16) Uani 1 1 d . . .
Ge2 Ge 0.24484(4) 0.2500 0.58580(6) 0.00922(18) Uani 1 2 d S . .
O1 O 0.2961(2) 0.2500 0.8421(6) 0.0163(7) Uani 1 2 d S . .
O2 O 0.46856(18) 0.1305(2) 0.6401(4) 0.0162(5) Uani 1 1 d . . .
O3 O 0.45841(16) 0.12634(19) 0.1664(4) 0.0166(5) Uani 1 1 d . . .
O4 O 0.2816(2) 0.14814(19) 0.4235(3) 0.0165(6) Uani 1 1 d . . .
O5 O 0.3678(2) -0.0269(2) 0.4140(3) 0.0179(6) Uani 1 1 d . . .
H1 H 0.4223 -0.0610 0.3981 0.027 Uiso 1 1 d R . .
O6 O 0.1206(3) 0.2500 0.5729(5) 0.0205(9) Uani 1 2 d S . .
K1 K 0.13545(9) 0.01650(8) 0.41099(12) 0.0307(3) Uani 1 1 d . . .
K2 K 0.13076(11) 0.2500 0.08235(16) 0.0275(3) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Gd1 O6 2.226(4) 6_657 ?
Gd1 O1 2.259(3) . ?
Gd1 O3 2.292(2) 8_566 ?
Gd1 O3 2.292(2) 1_556 ?
Gd1 O2 2.332(3) . ?
Gd1 O2 2.332(3) 8_565 ?
Gd1 K2 3.8249(12) 6_656 ?
Gd1 K1 3.8666(11) 2 ?
Gd1 K1 3.8666(11) 7_666 ?
Gd1 K2 3.8769(12) 6_657 ?
Gd1 K1 4.1548(13) 3_556 ?
Gd1 K1 4.1548(13) 6_657 ?
Ge1 O3 1.712(2) . ?
Ge1 O2 1.736(2) . ?
Ge1 O4 1.763(3) . ?
Ge1 O5 1.791(3) . ?
Ge1 K1 3.4571(9) 2_554 ?
Ge1 K1 3.4786(9) 2 ?
Ge1 K2 3.7603(13) 6_656 ?
Ge1 K1 3.8070(11) . ?
Ge1 K1 3.9242(12) 6_656 ?
Ge2 O1 1.709(3) . ?
Ge2 O6 1.702(4) . ?
Ge2 O4 1.781(2) . ?
Ge2 O4 1.781(2) 8_565 ?
Ge2 K2 3.3999(12) 1_556 ?
Ge2 K2 3.4372(12) . ?
Ge2 K1 3.6864(10) . ?
Ge2 K1 3.6864(10) 8_565 ?
O1 K2 2.694(3) 1_556 ?
O2 K1 2.965(3) 2 ?
O2 K2 3.072(3) 6_656 ?
O3 Gd1 2.292(2) 1_554 ?
O3 K1 2.808(3) 2_554 ?
O3 K1 2.890(3) 6_656 ?
O3 K2 3.281(3) 6_656 ?
O4 K1 2.694(3) . ?
O4 K2 3.243(3) . ?
O5 K1 3.026(2) 2 ?
O5 K1 3.063(2) 2_554 ?
O5 K2 3.222(3) 2 ?
O5 K1 3.235(3) . ?
O5 H1 0.8856 . ?
O6 Gd1 2.226(4) 6_557 ?
O6 K2 2.986(3) . ?
O6 K2 3.102(3) 1_556 ?
O6 K1 3.3507(15) . ?
O6 K1 3.3507(15) 8_565 ?
K1 O3 2.808(3) 2 ?
K1 O3 2.890(3) 6_556 ?
K1 O2 2.965(3) 2_554 ?
K1 O5 3.026(2) 2_554 ?
K1 O5 3.063(2) 2 ?
K1 Ge1 3.4571(9) 2 ?
K1 Ge1 3.4786(9) 2_554 ?
K1 K2 3.7705(11) . ?
K2 O1 2.694(3) 1_554 ?
K2 O2 3.072(3) 6_556 ?
K2 O2 3.072(3) 3_455 ?
K2 O6 3.102(3) 1_554 ?
K2 O5 3.222(3) 2_554 ?
K2 O5 3.222(3) 7_665 ?
K2 O4 3.243(3) 8_565 ?
K2 O3 3.281(3) 6_556 ?
K2 O3 3.281(3) 3_455 ?
K2 Ge2 3.3999(12) 1_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Gd1 O1 171.44(11) 6_657 . ?
O6 Gd1 O3 88.34(8) 6_657 8_566 ?
O1 Gd1 O3 97.41(8) . 8_566 ?
O6 Gd1 O3 88.34(8) 6_657 1_556 ?
O1 Gd1 O3 97.41(8) . 1_556 ?
O3 Gd1 O3 95.20(13) 8_566 1_556 ?
O6 Gd1 O2 88.16(8) 6_657 . ?
O1 Gd1 O2 85.74(9) . . ?
O3 Gd1 O2 175.37(9) 8_566 . ?
O3 Gd1 O2 87.73(11) 1_556 . ?
O6 Gd1 O2 88.16(8) 6_657 8_565 ?
O1 Gd1 O2 85.74(9) . 8_565 ?
O3 Gd1 O2 87.73(11) 8_566 8_565 ?
O3 Gd1 O2 175.37(9) 1_556 8_565 ?
O2 Gd1 O2 89.12(13) . 8_565 ?
O6 Gd1 K2 54.19(8) 6_657 6_656 ?
O1 Gd1 K2 117.25(9) . 6_656 ?
O3 Gd1 K2 121.96(6) 8_566 6_656 ?
O3 Gd1 K2 121.96(6) 1_556 6_656 ?
O2 Gd1 K2 53.42(7) . 6_656 ?
O2 Gd1 K2 53.42(7) 8_565 6_656 ?
O6 Gd1 K1 109.343(19) 6_657 2 ?
O1 Gd1 K1 70.99(2) . 2 ?
O3 Gd1 K1 134.31(7) 8_566 2 ?
O3 Gd1 K1 45.98(6) 1_556 2 ?
O2 Gd1 K1 49.97(7) . 2 ?
O2 Gd1 K1 132.91(7) 8_565 2 ?
K2 Gd1 K1 101.721(15) 6_656 2 ?
O6 Gd1 K1 109.343(19) 6_657 7_666 ?
O1 Gd1 K1 70.99(2) . 7_666 ?
O3 Gd1 K1 45.98(6) 8_566 7_666 ?
O3 Gd1 K1 134.31(6) 1_556 7_666 ?
O2 Gd1 K1 132.91(7) . 7_666 ?
O2 Gd1 K1 49.97(7) 8_565 7_666 ?
K2 Gd1 K1 101.721(15) 6_656 7_666 ?
K1 Gd1 K1 141.29(4) 2 7_666 ?
O6 Gd1 K2 50.12(8) 6_657 6_657 ?
O1 Gd1 K2 138.44(9) . 6_657 ?
O3 Gd1 K2 57.62(6) 8_566 6_657 ?
O3 Gd1 K2 57.62(6) 1_556 6_657 ?
O2 Gd1 K2 121.71(6) . 6_657 ?
O2 Gd1 K2 121.71(6) 8_565 6_657 ?
K2 Gd1 K2 104.31(4) 6_656 6_657 ?
K1 Gd1 K2 101.742(16) 2 6_657 ?
K1 Gd1 K2 101.742(16) 7_666 6_657 ?
O6 Gd1 K1 53.55(3) 6_657 3_556 ?
O1 Gd1 K1 128.50(2) . 3_556 ?
O3 Gd1 K1 41.97(6) 8_566 3_556 ?
O3 Gd1 K1 113.13(6) 1_556 3_556 ?
O2 Gd1 K1 133.46(7) . 3_556 ?
O2 Gd1 K1 66.93(6) 8_565 3_556 ?
K2 Gd1 K1 80.953(17) 6_656 3_556 ?
K1 Gd1 K1 156.918(16) 2 3_556 ?
K1 Gd1 K1 57.87(3) 7_666 3_556 ?
K2 Gd1 K1 55.869(14) 6_657 3_556 ?
O6 Gd1 K1 53.55(3) 6_657 6_657 ?
O1 Gd1 K1 128.50(2) . 6_657 ?
O3 Gd1 K1 113.13(6) 8_566 6_657 ?
O3 Gd1 K1 41.97(6) 1_556 6_657 ?
O2 Gd1 K1 66.93(6) . 6_657 ?
O2 Gd1 K1 133.46(6) 8_565 6_657 ?
K2 Gd1 K1 80.953(17) 6_656 6_657 ?
K1 Gd1 K1 57.87(3) 2 6_657 ?
K1 Gd1 K1 156.918(16) 7_666 6_657 ?
K2 Gd1 K1 55.869(14) 6_657 6_657 ?
K1 Gd1 K1 100.59(3) 3_556 6_657 ?
O3 Ge1 O2 113.61(13) . . ?
O3 Ge1 O4 112.90(10) . . ?
O2 Ge1 O4 111.25(10) . . ?
O3 Ge1 O5 109.68(12) . . ?
O2 Ge1 O5 110.83(12) . . ?
O4 Ge1 O5 97.42(13) . . ?
O3 Ge1 K1 53.77(9) . 2_554 ?
O2 Ge1 K1 153.88(9) . 2_554 ?
O4 Ge1 K1 94.82(7) . 2_554 ?
O5 Ge1 K1 62.19(7) . 2_554 ?
O3 Ge1 K1 156.86(9) . 2 ?
O2 Ge1 K1 58.42(9) . 2 ?
O4 Ge1 K1 89.76(7) . 2 ?
O5 Ge1 K1 60.43(7) . 2 ?
K1 Ge1 K1 122.55(3) 2_554 2 ?
O3 Ge1 K2 60.68(8) . 6_656 ?
O2 Ge1 K2 53.76(9) . 6_656 ?
O4 Ge1 K2 124.62(9) . 6_656 ?
O5 Ge1 K2 137.76(10) . 6_656 ?
K1 Ge1 K2 112.60(2) 2_554 6_656 ?
K1 Ge1 K2 110.94(2) 2 6_656 ?
O3 Ge1 K1 120.38(8) . . ?
O2 Ge1 K1 125.43(9) . . ?
O4 Ge1 K1 39.59(9) . . ?
O5 Ge1 K1 57.96(10) . . ?
K1 Ge1 K1 74.22(2) 2_554 . ?
K1 Ge1 K1 73.98(2) 2 . ?
K2 Ge1 K1 164.21(3) 6_656 . ?
O3 Ge1 K1 42.06(8) . 6_656 ?
O2 Ge1 K1 92.00(9) . 6_656 ?
O4 Ge1 K1 153.03(6) . 6_656 ?
O5 Ge1 K1 86.23(9) . 6_656 ?
K1 Ge1 K1 63.22(3) 2_554 6_656 ?
K1 Ge1 K1 114.795(18) 2 6_656 ?
K2 Ge1 K1 58.72(2) 6_656 6_656 ?
K1 Ge1 K1 134.07(2) . 6_656 ?
O1 Ge2 O6 116.90(15) . . ?
O1 Ge2 O4 112.91(9) . . ?
O6 Ge2 O4 104.88(11) . . ?
O1 Ge2 O4 112.91(9) . 8_565 ?
O6 Ge2 O4 104.88(11) . 8_565 ?
O4 Ge2 O4 103.05(16) . 8_565 ?
O1 Ge2 K2 51.58(10) . 1_556 ?
O6 Ge2 K2 65.31(11) . 1_556 ?
O4 Ge2 K2 128.47(8) . 1_556 ?
O4 Ge2 K2 128.47(8) 8_565 1_556 ?
O1 Ge2 K2 177.22(11) . . ?
O6 Ge2 K2 60.33(11) . . ?
O4 Ge2 K2 68.58(8) . . ?
O4 Ge2 K2 68.58(8) 8_565 . ?
K2 Ge2 K2 125.64(5) 1_556 . ?
O1 Ge2 K1 115.45(3) . . ?
O6 Ge2 K1 65.22(4) . . ?
O4 Ge2 K1 43.63(9) . . ?
O4 Ge2 K1 129.33(7) 8_565 . ?
K2 Ge2 K1 93.99(2) 1_556 . ?
K2 Ge2 K1 63.803(17) . . ?
O1 Ge2 K1 115.45(3) . 8_565 ?
O6 Ge2 K1 65.22(4) . 8_565 ?
O4 Ge2 K1 129.33(7) . 8_565 ?
O4 Ge2 K1 43.63(9) 8_565 8_565 ?
K2 Ge2 K1 93.99(2) 1_556 8_565 ?
K2 Ge2 K1 63.803(17) . 8_565 ?
K1 Ge2 K1 120.25(4) . 8_565 ?
Ge2 O1 Gd1 125.14(17) . . ?
Ge2 O1 K2 98.61(13) . 1_556 ?
Gd1 O1 K2 136.26(15) . 1_556 ?
Ge1 O2 Gd1 135.44(14) . . ?
Ge1 O2 K1 91.66(10) . 2 ?
Gd1 O2 K1 93.00(9) . 2 ?
Ge1 O2 K2 99.12(11) . 6_656 ?
Gd1 O2 K2 89.03(8) . 6_656 ?
K1 O2 K2 162.42(10) 2 6_656 ?
Ge1 O3 Gd1 137.53(14) . 1_554 ?
Ge1 O3 K1 96.77(10) . 2_554 ?
Gd1 O3 K1 98.08(9) 1_554 2_554 ?
Ge1 O3 K1 114.56(11) . 6_656 ?
Gd1 O3 K1 106.00(8) 1_554 6_656 ?
K1 O3 K1 86.06(8) 2_554 6_656 ?
Ge1 O3 K2 92.26(10) . 6_656 ?
Gd1 O3 K2 86.22(7) 1_554 6_656 ?
K1 O3 K2 161.04(9) 2_554 6_656 ?
K1 O3 K2 75.02(6) 6_656 6_656 ?
Ge1 O4 Ge2 125.71(14) . . ?
Ge1 O4 K1 115.75(12) . . ?
Ge2 O4 K1 109.23(12) . . ?
Ge1 O4 K2 135.96(10) . . ?
Ge2 O4 K2 80.67(9) . . ?
K1 O4 K2 78.26(7) . . ?
Ge1 O5 K1 88.59(9) . 2 ?
Ge1 O5 K1 86.66(9) . 2_554 ?
K1 O5 K1 174.40(12) 2 2_554 ?
Ge1 O5 K2 157.10(13) . 2 ?
K1 O5 K2 74.16(6) 2 2 ?
K1 O5 K2 111.19(8) 2_554 2 ?
Ge1 O5 K1 94.05(11) . . ?
K1 O5 K1 89.00(7) 2 . ?
K1 O5 K1 88.37(7) 2_554 . ?
K2 O5 K1 100.47(8) 2 . ?
Ge1 O5 H1 107.2 . . ?
K1 O5 H1 98.4 2 . ?
K1 O5 H1 85.8 2_554 . ?
K2 O5 H1 61.9 2 . ?
K1 O5 H1 157.6 . . ?
Ge2 O6 Gd1 175.01(18) . 6_557 ?
Ge2 O6 K2 89.99(14) . . ?
Gd1 O6 K2 94.99(12) 6_557 . ?
Ge2 O6 K2 84.79(13) . 1_556 ?
Gd1 O6 K2 90.22(11) 6_557 1_556 ?
K2 O6 K2 174.78(17) . 1_556 ?
Ge2 O6 K1 87.31(8) . . ?
Gd1 O6 K1 94.15(8) 6_557 . ?
K2 O6 K1 72.77(5) . . ?
K2 O6 K1 106.91(5) 1_556 . ?
Ge2 O6 K1 87.31(8) . 8_565 ?
Gd1 O6 K1 94.15(8) 6_557 8_565 ?
K2 O6 K1 72.77(5) . 8_565 ?
K2 O6 K1 106.91(5) 1_556 8_565 ?
K1 O6 K1 145.09(10) . 8_565 ?
O4 K1 O3 142.18(7) . 2 ?
O4 K1 O3 106.22(9) . 6_556 ?
O3 K1 O3 93.94(8) 2 6_556 ?
O4 K1 O2 145.73(7) . 2_554 ?
O3 K1 O2 67.37(8) 2 2_554 ?
O3 K1 O2 81.95(8) 6_556 2_554 ?
O4 K1 O5 90.45(7) . 2_554 ?
O3 K1 O5 125.33(8) 2 2_554 ?
O3 K1 O5 78.50(8) 6_556 2_554 ?
O2 K1 O5 57.97(7) 2_554 2_554 ?
O4 K1 O5 87.23(7) . 2 ?
O3 K1 O5 58.21(7) 2 2 ?
O3 K1 O5 97.26(8) 6_556 2 ?
O2 K1 O5 125.42(8) 2_554 2 ?
O5 K1 O5 174.40(12) 2_554 2 ?
O4 K1 O5 52.58(7) . . ?
O3 K1 O5 108.60(7) 2 . ?
O3 K1 O5 157.00(7) 6_556 . ?
O2 K1 O5 110.53(7) 2_554 . ?
O5 K1 O5 91.65(7) 2_554 . ?
O5 K1 O5 90.98(7) 2 . ?
O4 K1 O6 53.02(9) . . ?
O3 K1 O6 118.29(8) 2 . ?
O3 K1 O6 60.06(9) 6_556 . ?
O2 K1 O6 141.41(9) 2_554 . ?
O5 K1 O6 104.35(8) 2_554 . ?
O5 K1 O6 70.21(8) 2 . ?
O5 K1 O6 103.46(9) . . ?
O4 K1 Ge1 112.94(5) . 2 ?
O3 K1 Ge1 29.46(5) 2 2 ?
O3 K1 Ge1 105.16(6) 6_556 2 ?
O2 K1 Ge1 96.06(6) 2_554 2 ?
O5 K1 Ge1 153.44(7) 2_554 2 ?
O5 K1 Ge1 31.14(5) 2 2 ?
O5 K1 Ge1 92.97(4) . 2 ?
O6 K1 Ge1 99.96(6) . 2 ?
O4 K1 Ge1 115.90(5) . 2_554 ?
O3 K1 Ge1 95.84(6) 2 2_554 ?
O3 K1 Ge1 88.58(5) 6_556 2_554 ?
O2 K1 Ge1 29.92(5) 2_554 2_554 ?
O5 K1 Ge1 30.98(5) 2_554 2_554 ?
O5 K1 Ge1 153.61(7) 2 2_554 ?
O5 K1 Ge1 93.52(5) . 2_554 ?
O6 K1 Ge1 133.28(6) . 2_554 ?
Ge1 K1 Ge1 122.55(3) 2 2_554 ?
O4 K1 Ge2 27.14(5) . . ?
O3 K1 Ge2 129.05(6) 2 . ?
O3 K1 Ge2 86.35(6) 6_556 . ?
O2 K1 Ge2 160.69(6) 2_554 . ?
O5 K1 Ge2 104.68(6) 2_554 . ?
O5 K1 Ge2 71.20(6) 2 . ?
O5 K1 Ge2 76.00(5) . . ?
O6 K1 Ge2 27.46(7) . . ?
Ge1 K1 Ge2 101.81(2) 2 . ?
Ge1 K1 Ge2 135.05(3) 2_554 . ?
O4 K1 K2 57.35(6) . . ?
O3 K1 K2 151.12(7) 2 . ?
O3 K1 K2 57.21(6) 6_556 . ?
O2 K1 K2 105.81(6) 2_554 . ?
O5 K1 K2 55.29(6) 2_554 . ?
O5 K1 K2 119.34(7) 2 . ?
O5 K1 K2 100.10(5) . . ?
O6 K1 K2 49.16(5) . . ?
Ge1 K1 K2 148.44(4) 2 . ?
Ge1 K1 K2 85.41(2) 2_554 . ?
Ge2 K1 K2 54.88(2) . . ?
O1 K2 O6 125.51(11) 1_554 . ?
O1 K2 O2 111.61(8) 1_554 6_556 ?
O6 K2 O2 113.98(9) . 6_556 ?
O1 K2 O2 111.61(8) 1_554 3_455 ?
O6 K2 O2 113.98(9) . 3_455 ?
O2 K2 O2 64.37(10) 6_556 3_455 ?
O1 K2 O6 59.71(11) 1_554 1_554 ?
O6 K2 O6 174.78(17) . 1_554 ?
O2 K2 O6 61.82(8) 6_556 1_554 ?
O2 K2 O6 61.82(8) 3_455 1_554 ?
O1 K2 O5 79.77(6) 1_554 2_554 ?
O6 K2 O5 108.53(4) . 2_554 ?
O2 K2 O5 50.17(7) 6_556 2_554 ?
O2 K2 O5 111.68(7) 3_455 2_554 ?
O6 K2 O5 71.51(4) 1_554 2_554 ?
O1 K2 O5 79.77(6) 1_554 7_665 ?
O6 K2 O5 108.53(4) . 7_665 ?
O2 K2 O5 111.68(7) 6_556 7_665 ?
O2 K2 O5 50.17(7) 3_455 7_665 ?
O6 K2 O5 71.51(4) 1_554 7_665 ?
O5 K2 O5 142.93(8) 2_554 7_665 ?
O1 K2 O4 79.17(9) 1_554 8_565 ?
O6 K2 O4 52.43(8) . 8_565 ?
O2 K2 O4 166.20(7) 6_556 8_565 ?
O2 K2 O4 120.87(7) 3_455 8_565 ?
O6 K2 O4 131.89(8) 1_554 8_565 ?
O5 K2 O4 127.38(8) 2_554 8_565 ?
O5 K2 O4 77.98(6) 7_665 8_565 ?
O1 K2 O4 79.17(9) 1_554 . ?
O6 K2 O4 52.43(8) . . ?
O2 K2 O4 120.87(7) 6_556 . ?
O2 K2 O4 166.20(7) 3_455 . ?
O6 K2 O4 131.89(8) 1_554 . ?
O5 K2 O4 77.98(6) 2_554 . ?
O5 K2 O4 127.38(8) 7_665 . ?
O4 K2 O4 50.94(9) 8_565 . ?
O1 K2 O3 148.94(5) 1_554 6_556 ?
O6 K2 O3 60.09(8) . 6_556 ?
O2 K2 O3 53.89(7) 6_556 6_556 ?
O2 K2 O3 87.73(8) 3_455 6_556 ?
O6 K2 O3 115.67(8) 1_554 6_556 ?
O5 K2 O3 70.32(7) 2_554 6_556 ?
O5 K2 O3 129.91(8) 7_665 6_556 ?
O4 K2 O3 112.44(6) 8_565 6_556 ?
O4 K2 O3 86.45(7) . 6_556 ?
O1 K2 O3 148.94(5) 1_554 3_455 ?
O6 K2 O3 60.09(8) . 3_455 ?
O2 K2 O3 87.73(8) 6_556 3_455 ?
O2 K2 O3 53.89(7) 3_455 3_455 ?
O6 K2 O3 115.67(8) 1_554 3_455 ?
O5 K2 O3 129.91(8) 2_554 3_455 ?
O5 K2 O3 70.32(7) 7_665 3_455 ?
O4 K2 O3 86.45(7) 8_565 3_455 ?
O4 K2 O3 112.44(6) . 3_455 ?
O3 K2 O3 62.12(9) 6_556 3_455 ?
O1 K2 Ge2 29.81(7) 1_554 1_554 ?
O6 K2 Ge2 155.32(10) . 1_554 ?
O2 K2 Ge2 86.60(5) 6_556 1_554 ?
O2 K2 Ge2 86.60(5) 3_455 1_554 ?
O6 K2 Ge2 29.90(8) 1_554 1_554 ?
O5 K2 Ge2 73.43(5) 2_554 1_554 ?
O5 K2 Ge2 73.43(5) 7_665 1_554 ?
O4 K2 Ge2 106.01(6) 8_565 1_554 ?
O4 K2 Ge2 106.01(6) . 1_554 ?
O3 K2 Ge2 138.07(5) 6_556 1_554 ?
O3 K2 Ge2 138.07(5) 3_455 1_554 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O6 Ge2 O1 Gd1 180.0 . . . . ?
O4 Ge2 O1 Gd1 58.20(10) . . . . ?
O4 Ge2 O1 Gd1 -58.20(10) 8_565 . . . ?
K2 Ge2 O1 Gd1 180.0 1_556 . . . ?
K2 Ge2 O1 Gd1 180.000(8) . . . . ?
K1 Ge2 O1 Gd1 106.20(5) . . . . ?
K1 Ge2 O1 Gd1 -106.20(5) 8_565 . . . ?
O6 Ge2 O1 K2 0.0 . . . 1_556 ?
O4 Ge2 O1 K2 -121.80(10) . . . 1_556 ?
O4 Ge2 O1 K2 121.80(10) 8_565 . . 1_556 ?
K2 Ge2 O1 K2 0.000(8) . . . 1_556 ?
K1 Ge2 O1 K2 -73.80(5) . . . 1_556 ?
K1 Ge2 O1 K2 73.80(5) 8_565 . . 1_556 ?
O6 Gd1 O1 Ge2 0.000(2) 6_657 . . . ?
O3 Gd1 O1 Ge2 131.87(7) 8_566 . . . ?
O3 Gd1 O1 Ge2 -131.87(7) 1_556 . . . ?
O2 Gd1 O1 Ge2 -44.72(7) . . . . ?
O2 Gd1 O1 Ge2 44.72(7) 8_565 . . . ?
K2 Gd1 O1 Ge2 0.0 6_656 . . . ?
K1 Gd1 O1 Ge2 -93.68(3) 2 . . . ?
K1 Gd1 O1 Ge2 93.68(3) 7_666 . . . ?
K2 Gd1 O1 Ge2 180.0 6_657 . . . ?
K1 Gd1 O1 Ge2 100.58(7) 3_556 . . . ?
K1 Gd1 O1 Ge2 -100.58(7) 6_657 . . . ?
O6 Gd1 O1 K2 180.000(2) 6_657 . . 1_556 ?
O3 Gd1 O1 K2 -48.13(7) 8_566 . . 1_556 ?
O3 Gd1 O1 K2 48.13(7) 1_556 . . 1_556 ?
O2 Gd1 O1 K2 135.28(7) . . . 1_556 ?
O2 Gd1 O1 K2 -135.28(7) 8_565 . . 1_556 ?
K2 Gd1 O1 K2 180.0 6_656 . . 1_556 ?
K1 Gd1 O1 K2 86.32(3) 2 . . 1_556 ?
K1 Gd1 O1 K2 -86.32(3) 7_666 . . 1_556 ?
K2 Gd1 O1 K2 0.0 6_657 . . 1_556 ?
K1 Gd1 O1 K2 -79.42(7) 3_556 . . 1_556 ?
K1 Gd1 O1 K2 79.42(7) 6_657 . . 1_556 ?
O3 Ge1 O2 Gd1 108.62(19) . . . . ?
O4 Ge1 O2 Gd1 -20.1(2) . . . . ?
O5 Ge1 O2 Gd1 -127.4(2) . . . . ?
K1 Ge1 O2 Gd1 163.61(7) 2_554 . . . ?
K1 Ge1 O2 Gd1 -96.0(2) 2 . . . ?
K2 Ge1 O2 Gd1 98.0(2) 6_656 . . . ?
K1 Ge1 O2 Gd1 -62.6(2) . . . . ?
K1 Ge1 O2 Gd1 145.92(18) 6_656 . . . ?
O3 Ge1 O2 K1 -155.41(10) . . . 2 ?
O4 Ge1 O2 K1 75.86(11) . . . 2 ?
O5 Ge1 O2 K1 -31.38(13) . . . 2 ?
K1 Ge1 O2 K1 -100.42(19) 2_554 . . 2 ?
K2 Ge1 O2 K1 -166.06(12) 6_656 . . 2 ?
K1 Ge1 O2 K1 33.42(12) . . . 2 ?
K1 Ge1 O2 K1 -118.11(5) 6_656 . . 2 ?
O3 Ge1 O2 K2 10.66(16) . . . 6_656 ?
O4 Ge1 O2 K2 -118.08(11) . . . 6_656 ?
O5 Ge1 O2 K2 134.68(11) . . . 6_656 ?
K1 Ge1 O2 K2 65.6(2) 2_554 . . 6_656 ?
K1 Ge1 O2 K2 166.06(12) 2 . . 6_656 ?
K1 Ge1 O2 K2 -160.52(4) . . . 6_656 ?
K1 Ge1 O2 K2 47.96(7) 6_656 . . 6_656 ?
O6 Gd1 O2 Ge1 -147.2(2) 6_657 . . . ?
O1 Gd1 O2 Ge1 26.8(2) . . . . ?
O3 Gd1 O2 Ge1 -106.2(11) 8_566 . . . ?
O3 Gd1 O2 Ge1 124.39(19) 1_556 . . . ?
O2 Gd1 O2 Ge1 -59.0(2) 8_565 . . . ?
K2 Gd1 O2 Ge1 -102.0(2) 6_656 . . . ?
K1 Gd1 O2 Ge1 95.4(2) 2 . . . ?
K1 Gd1 O2 Ge1 -32.2(2) 7_666 . . . ?
K2 Gd1 O2 Ge1 173.50(16) 6_657 . . . ?
K1 Gd1 O2 Ge1 -115.35(17) 3_556 . . . ?
K1 Gd1 O2 Ge1 162.0(2) 6_657 . . . ?
O6 Gd1 O2 K1 117.37(8) 6_657 . . 2 ?
O1 Gd1 O2 K1 -68.64(8) . . . 2 ?
O3 Gd1 O2 K1 158.4(10) 8_566 . . 2 ?
O3 Gd1 O2 K1 28.96(9) 1_556 . . 2 ?
O2 Gd1 O2 K1 -154.44(4) 8_565 . . 2 ?
K2 Gd1 O2 K1 162.52(10) 6_656 . . 2 ?
K1 Gd1 O2 K1 -127.63(7) 7_666 . . 2 ?
K2 Gd1 O2 K1 78.08(8) 6_657 . . 2 ?
K1 Gd1 O2 K1 149.22(4) 3_556 . . 2 ?
K1 Gd1 O2 K1 66.60(6) 6_657 . . 2 ?
O6 Gd1 O2 K2 -45.15(7) 6_657 . . 6_656 ?
O1 Gd1 O2 K2 128.83(8) . . . 6_656 ?
O3 Gd1 O2 K2 -4.2(11) 8_566 . . 6_656 ?
O3 Gd1 O2 K2 -133.57(7) 1_556 . . 6_656 ?
O2 Gd1 O2 K2 43.03(10) 8_565 . . 6_656 ?
K1 Gd1 O2 K2 -162.52(10) 2 . . 6_656 ?
K1 Gd1 O2 K2 69.85(9) 7_666 . . 6_656 ?
K2 Gd1 O2 K2 -84.45(8) 6_657 . . 6_656 ?
K1 Gd1 O2 K2 -13.30(11) 3_556 . . 6_656 ?
K1 Gd1 O2 K2 -95.92(6) 6_657 . . 6_656 ?
O2 Ge1 O3 Gd1 -96.7(2) . . . 1_554 ?
O4 Ge1 O3 Gd1 31.2(2) . . . 1_554 ?
O5 Ge1 O3 Gd1 138.63(19) . . . 1_554 ?
K1 Ge1 O3 Gd1 109.8(2) 2_554 . . 1_554 ?
K1 Ge1 O3 Gd1 -161.15(8) 2 . . 1_554 ?
K2 Ge1 O3 Gd1 -86.87(19) 6_656 . . 1_554 ?
K1 Ge1 O3 Gd1 74.9(2) . . . 1_554 ?
K1 Ge1 O3 Gd1 -161.4(3) 6_656 . . 1_554 ?
O2 Ge1 O3 K1 153.45(10) . . . 2_554 ?
O4 Ge1 O3 K1 -78.66(12) . . . 2_554 ?
O5 Ge1 O3 K1 28.80(13) . . . 2_554 ?
K1 Ge1 O3 K1 89.0(2) 2 . . 2_554 ?
K2 Ge1 O3 K1 163.30(11) 6_656 . . 2_554 ?
K1 Ge1 O3 K1 -34.88(11) . . . 2_554 ?
K1 Ge1 O3 K1 88.75(12) 6_656 . . 2_554 ?
O2 Ge1 O3 K1 64.70(17) . . . 6_656 ?
O4 Ge1 O3 K1 -167.42(10) . . . 6_656 ?
O5 Ge1 O3 K1 -59.95(15) . . . 6_656 ?
K1 Ge1 O3 K1 -88.75(12) 2_554 . . 6_656 ?
K1 Ge1 O3 K1 0.3(3) 2 . . 6_656 ?
K2 Ge1 O3 K1 74.54(9) 6_656 . . 6_656 ?
K1 Ge1 O3 K1 -123.64(8) . . . 6_656 ?
O2 Ge1 O3 K2 -9.85(15) . . . 6_656 ?
O4 Ge1 O3 K2 118.04(10) . . . 6_656 ?
O5 Ge1 O3 K2 -134.50(11) . . . 6_656 ?
K1 Ge1 O3 K2 -163.30(11) 2_554 . . 6_656 ?
K1 Ge1 O3 K2 -74.3(2) 2 . . 6_656 ?
K1 Ge1 O3 K2 161.82(3) . . . 6_656 ?
K1 Ge1 O3 K2 -74.54(9) 6_656 . . 6_656 ?
O3 Ge1 O4 Ge2 -106.63(16) . . . . ?
O2 Ge1 O4 Ge2 22.5(2) . . . . ?
O5 Ge1 O4 Ge2 138.30(16) . . . . ?
K1 Ge1 O4 Ge2 -159.17(14) 2_554 . . . ?
K1 Ge1 O4 Ge2 78.18(15) 2 . . . ?
K2 Ge1 O4 Ge2 -37.38(18) 6_656 . . . ?
K1 Ge1 O4 Ge2 142.8(2) . . . . ?
K1 Ge1 O4 Ge2 -125.40(12) 6_656 . . . ?
O3 Ge1 O4 K1 110.52(13) . . . . ?
O2 Ge1 O4 K1 -120.37(12) . . . . ?
O5 Ge1 O4 K1 -4.55(10) . . . . ?
K1 Ge1 O4 K1 57.99(8) 2_554 . . . ?
K1 Ge1 O4 K1 -64.67(8) 2 . . . ?
K2 Ge1 O4 K1 179.78(4) 6_656 . . . ?
K1 Ge1 O4 K1 91.75(19) 6_656 . . . ?
O3 Ge1 O4 K2 10.5(2) . . . . ?
O2 Ge1 O4 K2 139.62(16) . . . . ?
O5 Ge1 O4 K2 -104.56(16) . . . . ?
K1 Ge1 O4 K2 -42.02(16) 2_554 . . . ?
K1 Ge1 O4 K2 -164.68(15) 2 . . . ?
K2 Ge1 O4 K2 79.77(16) 6_656 . . . ?
K1 Ge1 O4 K2 -100.01(17) . . . . ?
K1 Ge1 O4 K2 -8.3(3) 6_656 . . . ?
O1 Ge2 O4 Ge1 -41.4(2) . . . . ?
O6 Ge2 O4 Ge1 -169.70(16) . . . . ?
O4 Ge2 O4 Ge1 80.76(18) 8_565 . . . ?
K2 Ge2 O4 Ge1 -99.63(17) 1_556 . . . ?
K2 Ge2 O4 Ge1 141.18(18) . . . . ?
K1 Ge2 O4 Ge1 -144.8(2) . . . . ?
K1 Ge2 O4 Ge1 120.35(13) 8_565 . . . ?
O1 Ge2 O4 K1 103.47(13) . . . . ?
O6 Ge2 O4 K1 -24.88(13) . . . . ?
O4 Ge2 O4 K1 -134.41(8) 8_565 . . . ?
K2 Ge2 O4 K1 45.19(13) 1_556 . . . ?
K2 Ge2 O4 K1 -74.00(8) . . . . ?
K1 Ge2 O4 K1 -94.83(11) 8_565 . . . ?
O1 Ge2 O4 K2 177.46(10) . . . . ?
O6 Ge2 O4 K2 49.12(10) . . . . ?
O4 Ge2 O4 K2 -60.42(13) 8_565 . . . ?
K2 Ge2 O4 K2 119.19(8) 1_556 . . . ?
K1 Ge2 O4 K2 74.00(8) . . . . ?
K1 Ge2 O4 K2 -20.83(11) 8_565 . . . ?
O3 Ge1 O5 K1 156.91(9) . . . 2 ?
O2 Ge1 O5 K1 30.67(13) . . . 2 ?
O4 Ge1 O5 K1 -85.48(9) . . . 2 ?
K1 Ge1 O5 K1 -177.03(12) 2_554 . . 2 ?
K2 Ge1 O5 K1 89.22(10) 6_656 . . 2 ?
K1 Ge1 O5 K1 -88.90(7) . . . 2 ?
K1 Ge1 O5 K1 121.38(6) 6_656 . . 2 ?
O3 Ge1 O5 K1 -26.06(12) . . . 2_554 ?
O2 Ge1 O5 K1 -152.30(9) . . . 2_554 ?
O4 Ge1 O5 K1 91.55(8) . . . 2_554 ?
K1 Ge1 O5 K1 177.03(12) 2 . . 2_554 ?
K2 Ge1 O5 K1 -93.75(9) 6_656 . . 2_554 ?
K1 Ge1 O5 K1 88.13(7) . . . 2_554 ?
K1 Ge1 O5 K1 -61.60(6) 6_656 . . 2_554 ?
O3 Ge1 O5 K2 116.3(3) . . . 2 ?
O2 Ge1 O5 K2 -9.9(4) . . . 2 ?
O4 Ge1 O5 K2 -126.1(3) . . . 2 ?
K1 Ge1 O5 K2 142.4(4) 2_554 . . 2 ?
K1 Ge1 O5 K2 -40.6(3) 2 . . 2 ?
K2 Ge1 O5 K2 48.6(4) 6_656 . . 2 ?
K1 Ge1 O5 K2 -129.5(3) . . . 2 ?
K1 Ge1 O5 K2 80.8(3) 6_656 . . 2 ?
O3 Ge1 O5 K1 -114.19(9) . . . . ?
O2 Ge1 O5 K1 119.57(10) . . . . ?
O4 Ge1 O5 K1 3.42(8) . . . . ?
K1 Ge1 O5 K1 -88.13(7) 2_554 . . . ?
K1 Ge1 O5 K1 88.90(7) 2 . . . ?
K2 Ge1 O5 K1 178.12(5) 6_656 . . . ?
K1 Ge1 O5 K1 -149.72(4) 6_656 . . . ?
O1 Ge2 O6 Gd1 0.000(3) . . . 6_557 ?
O4 Ge2 O6 Gd1 125.90(8) . . . 6_557 ?
O4 Ge2 O6 Gd1 -125.90(8) 8_565 . . 6_557 ?
K2 Ge2 O6 Gd1 0.000(3) 1_556 . . 6_557 ?
K2 Ge2 O6 Gd1 180.000(3) . . . 6_557 ?
K1 Ge2 O6 Gd1 107.25(5) . . . 6_557 ?
K1 Ge2 O6 Gd1 -107.25(5) 8_565 . . 6_557 ?
O1 Ge2 O6 K2 180.0 . . . . ?
O4 Ge2 O6 K2 -54.10(8) . . . . ?
O4 Ge2 O6 K2 54.10(8) 8_565 . . . ?
K2 Ge2 O6 K2 180.0 1_556 . . . ?
K1 Ge2 O6 K2 -72.75(5) . . . . ?
K1 Ge2 O6 K2 72.75(5) 8_565 . . . ?
O1 Ge2 O6 K2 0.0 . . . 1_556 ?
O4 Ge2 O6 K2 125.90(8) . . . 1_556 ?
O4 Ge2 O6 K2 -125.90(8) 8_565 . . 1_556 ?
K2 Ge2 O6 K2 180.0 . . . 1_556 ?
K1 Ge2 O6 K2 107.25(5) . . . 1_556 ?
K1 Ge2 O6 K2 -107.25(5) 8_565 . . 1_556 ?
O1 Ge2 O6 K1 -107.25(5) . . . . ?
O4 Ge2 O6 K1 18.65(10) . . . . ?
O4 Ge2 O6 K1 126.85(8) 8_565 . . . ?
K2 Ge2 O6 K1 -107.25(5) 1_556 . . . ?
K2 Ge2 O6 K1 72.75(5) . . . . ?
K1 Ge2 O6 K1 145.49(9) 8_565 . . . ?
O1 Ge2 O6 K1 107.25(5) . . . 8_565 ?
O4 Ge2 O6 K1 -126.85(8) . . . 8_565 ?
O4 Ge2 O6 K1 -18.65(10) 8_565 . . 8_565 ?
K2 Ge2 O6 K1 107.25(5) 1_556 . . 8_565 ?
K2 Ge2 O6 K1 -72.75(5) . . . 8_565 ?
K1 Ge2 O6 K1 -145.49(9) . . . 8_565 ?
Ge1 O4 K1 O3 73.83(16) . . . 2 ?
Ge2 O4 K1 O3 -74.88(18) . . . 2 ?
K2 O4 K1 O3 -150.53(12) . . . 2 ?
Ge1 O4 K1 O3 -166.74(9) . . . 6_556 ?
Ge2 O4 K1 O3 44.55(11) . . . 6_556 ?
K2 O4 K1 O3 -31.10(7) . . . 6_556 ?
Ge1 O4 K1 O2 -67.08(19) . . . 2_554 ?
Ge2 O4 K1 O2 144.21(13) . . . 2_554 ?
K2 O4 K1 O2 68.56(16) . . . 2_554 ?
Ge1 O4 K1 O5 -88.59(11) . . . 2_554 ?
Ge2 O4 K1 O5 122.70(11) . . . 2_554 ?
K2 O4 K1 O5 47.05(7) . . . 2_554 ?
Ge1 O4 K1 O5 96.51(11) . . . 2 ?
Ge2 O4 K1 O5 -52.21(11) . . . 2 ?
K2 O4 K1 O5 -127.86(7) . . . 2 ?
Ge1 O4 K1 O5 3.14(7) . . . . ?
Ge2 O4 K1 O5 -145.57(13) . . . . ?
K2 O4 K1 O5 138.78(7) . . . . ?
Ge1 O4 K1 O6 163.69(14) . . . . ?
Ge2 O4 K1 O6 14.98(9) . . . . ?
K2 O4 K1 O6 -60.67(8) . . . . ?
Ge1 O4 K1 Ge1 78.49(10) . . . 2 ?
Ge2 O4 K1 Ge1 -70.22(11) . . . 2 ?
K2 O4 K1 Ge1 -145.87(5) . . . 2 ?
Ge1 O4 K1 Ge1 -70.27(11) . . . 2_554 ?
Ge2 O4 K1 Ge1 141.02(8) . . . 2_554 ?
K2 O4 K1 Ge1 65.37(6) . . . 2_554 ?
Ge1 O4 K1 Ge2 148.71(17) . . . . ?
K2 O4 K1 Ge2 -75.65(10) . . . . ?
Ge1 O4 K1 K2 -135.64(11) . . . . ?
Ge2 O4 K1 K2 75.65(10) . . . . ?
Ge1 O5 K1 O4 -2.79(6) . . . . ?
K1 O5 K1 O4 85.72(8) 2 . . . ?
K1 O5 K1 O4 -89.33(8) 2_554 . . . ?
K2 O5 K1 O4 159.42(9) 2 . . . ?
Ge1 O5 K1 O3 -145.17(8) . . . 2 ?
K1 O5 K1 O3 -56.65(8) 2 . . 2 ?
K1 O5 K1 O3 128.29(8) 2_554 . . 2 ?
K2 O5 K1 O3 17.05(8) 2 . . 2 ?
Ge1 O5 K1 O3 22.8(2) . . . 6_556 ?
K1 O5 K1 O3 111.30(16) 2 . . 6_556 ?
K1 O5 K1 O3 -63.76(18) 2_554 . . 6_556 ?
K2 O5 K1 O3 -175.01(14) 2 . . 6_556 ?
Ge1 O5 K1 O2 142.74(9) . . . 2_554 ?
K1 O5 K1 O2 -128.74(8) 2 . . 2_554 ?
K1 O5 K1 O2 56.20(8) 2_554 . . 2_554 ?
K2 O5 K1 O2 -55.04(8) 2 . . 2_554 ?
Ge1 O5 K1 O5 86.51(9) . . . 2_554 ?
K1 O5 K1 O5 175.03(11) 2 . . 2_554 ?
K1 O5 K1 O5 -0.030(3) 2_554 . . 2_554 ?
K2 O5 K1 O5 -111.28(9) 2 . . 2_554 ?
Ge1 O5 K1 O5 -88.55(9) . . . 2 ?
K1 O5 K1 O5 -0.030(4) 2 . . 2 ?
K1 O5 K1 O5 -175.09(11) 2_554 . . 2 ?
K2 O5 K1 O5 73.66(6) 2 . . 2 ?
Ge1 O5 K1 O6 -18.67(9) . . . . ?
K1 O5 K1 O6 69.85(8) 2 . . . ?
K1 O5 K1 O6 -105.21(8) 2_554 . . . ?
K2 O5 K1 O6 143.54(7) 2 . . . ?
Ge1 O5 K1 Ge1 -119.65(7) . . . 2 ?
K1 O5 K1 Ge1 -31.13(5) 2 . . 2 ?
K1 O5 K1 Ge1 153.81(7) 2_554 . . 2 ?
K2 O5 K1 Ge1 42.56(5) 2 . . 2 ?
Ge1 O5 K1 Ge1 117.46(7) . . . 2_554 ?
K1 O5 K1 Ge1 -154.02(7) 2 . . 2_554 ?
K1 O5 K1 Ge1 30.93(5) 2_554 . . 2_554 ?
K2 O5 K1 Ge1 -80.32(5) 2 . . 2_554 ?
Ge1 O5 K1 Ge2 -18.21(6) . . . . ?
K1 O5 K1 Ge2 70.31(5) 2 . . . ?
K1 O5 K1 Ge2 -104.75(6) 2_554 . . . ?
K2 O5 K1 Ge2 144.00(6) 2 . . . ?
Ge1 O5 K1 K2 31.51(8) . . . . ?
K1 O5 K1 K2 120.03(6) 2 . . . ?
K1 O5 K1 K2 -55.03(6) 2_554 . . . ?
K2 O5 K1 K2 -166.28(5) 2 . . . ?
Ge2 O6 K1 O4 -14.82(8) . . . . ?
Gd1 O6 K1 O4 169.96(13) 6_557 . . . ?
K2 O6 K1 O4 76.01(9) . . . . ?
K2 O6 K1 O4 -98.54(13) 1_556 . . . ?
K1 O6 K1 O4 66.6(2) 8_565 . . . ?
Ge2 O6 K1 O3 121.05(11) . . . 2 ?
Gd1 O6 K1 O3 -54.18(12) 6_557 . . 2 ?
K2 O6 K1 O3 -148.12(8) . . . 2 ?
K2 O6 K1 O3 37.32(15) 1_556 . . 2 ?
K1 O6 K1 O3 -157.5(2) 8_565 . . 2 ?
Ge2 O6 K1 O3 -161.67(14) . . . 6_556 ?
Gd1 O6 K1 O3 23.11(8) 6_557 . . 6_556 ?
K2 O6 K1 O3 -70.84(9) . . . 6_556 ?
K2 O6 K1 O3 114.61(14) 1_556 . . 6_556 ?
K1 O6 K1 O3 -80.2(2) 8_565 . . 6_556 ?
Ge2 O6 K1 O2 -150.45(11) . . . 2_554 ?
Gd1 O6 K1 O2 34.33(16) 6_557 . . 2_554 ?
K2 O6 K1 O2 -59.62(15) . . . 2_554 ?
K2 O6 K1 O2 125.83(12) 1_556 . . 2_554 ?
K1 O6 K1 O2 -69.0(3) 8_565 . . 2_554 ?
Ge2 O6 K1 O5 -94.30(12) . . . 2_554 ?
Gd1 O6 K1 O5 90.48(10) 6_557 . . 2_554 ?
K2 O6 K1 O5 -3.47(11) . . . 2_554 ?
K2 O6 K1 O5 -178.02(11) 1_556 . . 2_554 ?
K1 O6 K1 O5 -12.9(3) 8_565 . . 2_554 ?
Ge2 O6 K1 O5 87.10(12) . . . 2 ?
Gd1 O6 K1 O5 -88.13(10) 6_557 . . 2 ?
K2 O6 K1 O5 177.93(11) . . . 2 ?
K2 O6 K1 O5 3.37(10) 1_556 . . 2 ?
K1 O6 K1 O5 168.5(3) 8_565 . . 2 ?
Ge2 O6 K1 O5 0.97(12) . . . . ?
Gd1 O6 K1 O5 -174.26(8) 6_557 . . . ?
K2 O6 K1 O5 91.79(8) . . . . ?
K2 O6 K1 O5 -82.76(11) 1_556 . . . ?
K1 O6 K1 O5 82.4(2) 8_565 . . . ?
Ge2 O6 K1 Ge1 96.48(10) . . . 2 ?
Gd1 O6 K1 Ge1 -78.74(9) 6_557 . . 2 ?
K2 O6 K1 Ge1 -172.69(6) . . . 2 ?
K2 O6 K1 Ge1 12.76(12) 1_556 . . 2 ?
K1 O6 K1 Ge1 177.9(2) 8_565 . . 2 ?
Ge2 O6 K1 Ge1 -107.23(11) . . . 2_554 ?
Gd1 O6 K1 Ge1 77.55(12) 6_557 . . 2_554 ?
K2 O6 K1 Ge1 -16.40(14) . . . 2_554 ?
K2 O6 K1 Ge1 169.05(6) 1_556 . . 2_554 ?
K1 O6 K1 Ge1 -25.8(3) 8_565 . . 2_554 ?
Gd1 O6 K1 Ge2 -175.23(18) 6_557 . . . ?
K2 O6 K1 Ge2 90.83(12) . . . . ?
K2 O6 K1 Ge2 -83.73(14) 1_556 . . . ?
K1 O6 K1 Ge2 81.4(2) 8_565 . . . ?
Ge2 O6 K1 K2 -90.83(12) . . . . ?
Gd1 O6 K1 K2 93.95(11) 6_557 . . . ?
K2 O6 K1 K2 -174.55(17) 1_556 . . . ?
K1 O6 K1 K2 -9.41(18) 8_565 . . . ?
O1 Ge2 K1 O4 -97.21(15) . . . . ?
O6 Ge2 K1 O4 153.40(15) . . . . ?
O4 Ge2 K1 O4 64.12(15) 8_565 . . . ?
K2 Ge2 K1 O4 -146.17(11) 1_556 . . . ?
K2 Ge2 K1 O4 85.77(11) . . . . ?
K1 Ge2 K1 O4 116.85(11) 8_565 . . . ?
O1 Ge2 K1 O3 33.13(14) . . . 2 ?
O6 Ge2 K1 O3 -76.27(13) . . . 2 ?
O4 Ge2 K1 O3 130.34(13) . . . 2 ?
O4 Ge2 K1 O3 -165.55(14) 8_565 . . 2 ?
K2 Ge2 K1 O3 -15.83(8) 1_556 . . 2 ?
K2 Ge2 K1 O3 -143.90(9) . . . 2 ?
K1 Ge2 K1 O3 -112.81(7) 8_565 . . 2 ?
O1 Ge2 K1 O3 125.25(12) . . . 6_556 ?
O6 Ge2 K1 O3 15.85(12) . . . 6_556 ?
O4 Ge2 K1 O3 -137.55(12) . . . 6_556 ?
O4 Ge2 K1 O3 -73.43(13) 8_565 . . 6_556 ?
K2 Ge2 K1 O3 76.29(6) 1_556 . . 6_556 ?
K2 Ge2 K1 O3 -51.78(6) . . . 6_556 ?
K1 Ge2 K1 O3 -20.69(6) 8_565 . . 6_556 ?
O1 Ge2 K1 O2 177.9(2) . . . 2_554 ?
O6 Ge2 K1 O2 68.5(2) . . . 2_554 ?
O4 Ge2 K1 O2 -84.9(2) . . . 2_554 ?
O4 Ge2 K1 O2 -20.8(2) 8_565 . . 2_554 ?
K2 Ge2 K1 O2 128.96(19) 1_556 . . 2_554 ?
K2 Ge2 K1 O2 0.89(19) . . . 2_554 ?
K1 Ge2 K1 O2 32.0(2) 8_565 . . 2_554 ?
O1 Ge2 K1 O5 -157.65(12) . . . 2_554 ?
O6 Ge2 K1 O5 92.96(13) . . . 2_554 ?
O4 Ge2 K1 O5 -60.44(12) . . . 2_554 ?
O4 Ge2 K1 O5 3.67(14) 8_565 . . 2_554 ?
K2 Ge2 K1 O5 153.39(7) 1_556 . . 2_554 ?
K2 Ge2 K1 O5 25.32(7) . . . 2_554 ?
K1 Ge2 K1 O5 56.41(8) 8_565 . . 2_554 ?
O1 Ge2 K1 O5 26.30(13) . . . 2 ?
O6 Ge2 K1 O5 -83.09(13) . . . 2 ?
O4 Ge2 K1 O5 123.51(12) . . . 2 ?
O4 Ge2 K1 O5 -172.37(13) 8_565 . . 2 ?
K2 Ge2 K1 O5 -22.66(7) 1_556 . . 2 ?
K2 Ge2 K1 O5 -150.72(7) . . . 2 ?
K1 Ge2 K1 O5 -119.64(6) 8_565 . . 2 ?
O1 Ge2 K1 O5 -69.64(11) . . . . ?
O6 Ge2 K1 O5 -179.03(12) . . . . ?
O4 Ge2 K1 O5 27.57(11) . . . . ?
O4 Ge2 K1 O5 91.69(12) 8_565 . . . ?
K2 Ge2 K1 O5 -118.60(4) 1_556 . . . ?
K2 Ge2 K1 O5 113.34(5) . . . . ?
K1 Ge2 K1 O5 144.42(5) 8_565 . . . ?
O1 Ge2 K1 O6 109.40(15) . . . . ?
O4 Ge2 K1 O6 -153.40(15) . . . . ?
O4 Ge2 K1 O6 -89.28(16) 8_565 . . . ?
K2 Ge2 K1 O6 60.44(11) 1_556 . . . ?
K2 Ge2 K1 O6 -67.63(11) . . . . ?
K1 Ge2 K1 O6 -36.54(11) 8_565 . . . ?
O1 Ge2 K1 Ge1 20.50(11) . . . 2 ?
O6 Ge2 K1 Ge1 -88.89(11) . . . 2 ?
O4 Ge2 K1 Ge1 117.71(11) . . . 2 ?
O4 Ge2 K1 Ge1 -178.17(12) 8_565 . . 2 ?
K2 Ge2 K1 Ge1 -28.46(4) 1_556 . . 2 ?
K2 Ge2 K1 Ge1 -156.52(4) . . . 2 ?
K1 Ge2 K1 Ge1 -125.43(2) 8_565 . . 2 ?
O1 Ge2 K1 Ge1 -150.43(12) . . . 2_554 ?
O6 Ge2 K1 Ge1 100.18(12) . . . 2_554 ?
O4 Ge2 K1 Ge1 -53.22(11) . . . 2_554 ?
O4 Ge2 K1 Ge1 10.90(14) 8_565 . . 2_554 ?
K2 Ge2 K1 Ge1 160.61(5) 1_556 . . 2_554 ?
K2 Ge2 K1 Ge1 32.55(5) . . . 2_554 ?
K1 Ge2 K1 Ge1 63.63(7) 8_565 . . 2_554 ?
O1 Ge2 K1 K2 177.03(11) . . . . ?
O6 Ge2 K1 K2 67.63(11) . . . . ?
O4 Ge2 K1 K2 -85.77(11) . . . . ?
O4 Ge2 K1 K2 -21.65(12) 8_565 . . . ?
K2 Ge2 K1 K2 128.07(5) 1_556 . . . ?
K1 Ge2 K1 K2 31.09(4) 8_565 . . . ?
Ge2 O6 K2 O1 0.0 . . . 1_554 ?
Gd1 O6 K2 O1 180.0 6_557 . . 1_554 ?
K2 O6 K2 O1 0.000(3) 1_556 . . 1_554 ?
K1 O6 K2 O1 -87.19(5) . . . 1_554 ?
K1 O6 K2 O1 87.19(5) 8_565 . . 1_554 ?
Ge2 O6 K2 O2 144.34(6) . . . 6_556 ?
Gd1 O6 K2 O2 -35.66(6) 6_557 . . 6_556 ?
K2 O6 K2 O2 144.34(6) 1_556 . . 6_556 ?
K1 O6 K2 O2 57.15(9) . . . 6_556 ?
K1 O6 K2 O2 -128.47(7) 8_565 . . 6_556 ?
Ge2 O6 K2 O2 -144.34(6) . . . 3_455 ?
Gd1 O6 K2 O2 35.66(6) 6_557 . . 3_455 ?
K2 O6 K2 O2 -144.34(6) 1_556 . . 3_455 ?
K1 O6 K2 O2 128.47(7) . . . 3_455 ?
K1 O6 K2 O2 -57.15(9) 8_565 . . 3_455 ?
Ge2 O6 K2 O6 180.000(2) . . . 1_554 ?
Gd1 O6 K2 O6 0.000(1) 6_557 . . 1_554 ?
K2 O6 K2 O6 180.000(4) 1_556 . . 1_554 ?
K1 O6 K2 O6 92.81(5) . . . 1_554 ?
K1 O6 K2 O6 -92.81(5) 8_565 . . 1_554 ?
Ge2 O6 K2 O5 90.52(7) . . . 2_554 ?
Gd1 O6 K2 O5 -89.48(7) 6_557 . . 2_554 ?
K2 O6 K2 O5 90.52(7) 1_556 . . 2_554 ?
K1 O6 K2 O5 3.33(10) . . . 2_554 ?
K1 O6 K2 O5 177.71(7) 8_565 . . 2_554 ?
Ge2 O6 K2 O5 -90.52(7) . . . 7_665 ?
Gd1 O6 K2 O5 89.48(7) 6_557 . . 7_665 ?
K2 O6 K2 O5 -90.52(7) 1_556 . . 7_665 ?
K1 O6 K2 O5 -177.71(7) . . . 7_665 ?
K1 O6 K2 O5 -3.33(10) 8_565 . . 7_665 ?
Ge2 O6 K2 O4 -32.85(7) . . . 8_565 ?
Gd1 O6 K2 O4 147.15(7) 6_557 . . 8_565 ?
K2 O6 K2 O4 -32.85(7) 1_556 . . 8_565 ?
K1 O6 K2 O4 -120.04(10) . . . 8_565 ?
K1 O6 K2 O4 54.34(7) 8_565 . . 8_565 ?
Ge2 O6 K2 O4 32.85(7) . . . . ?
Gd1 O6 K2 O4 -147.15(7) 6_557 . . . ?
K2 O6 K2 O4 32.85(7) 1_556 . . . ?
K1 O6 K2 O4 -54.34(7) . . . . ?
K1 O6 K2 O4 120.04(10) 8_565 . . . ?
Ge2 O6 K2 O3 143.47(6) . . . 6_556 ?
Gd1 O6 K2 O3 -36.53(6) 6_557 . . 6_556 ?
K2 O6 K2 O3 143.47(6) 1_556 . . 6_556 ?
K1 O6 K2 O3 56.29(6) . . . 6_556 ?
K1 O6 K2 O3 -129.34(9) 8_565 . . 6_556 ?
Ge2 O6 K2 O3 -143.47(6) . . . 3_455 ?
Gd1 O6 K2 O3 36.53(6) 6_557 . . 3_455 ?
K2 O6 K2 O3 -143.48(6) 1_556 . . 3_455 ?
K1 O6 K2 O3 129.34(9) . . . 3_455 ?
K1 O6 K2 O3 -56.29(6) 8_565 . . 3_455 ?
Ge2 O6 K2 Ge2 0.0 . . . 1_554 ?
Gd1 O6 K2 Ge2 180.0 6_557 . . 1_554 ?
K2 O6 K2 Ge2 0.000(3) 1_556 . . 1_554 ?
K1 O6 K2 Ge2 -87.19(5) . . . 1_554 ?
K1 O6 K2 Ge2 87.19(5) 8_565 . . 1_554 ?
Ge1 O4 K2 O1 -11.33(16) . . . 1_554 ?
Ge2 O4 K2 O1 121.59(9) . . . 1_554 ?
K1 O4 K2 O1 -126.38(6) . . . 1_554 ?
Ge1 O4 K2 O6 -164.6(2) . . . . ?
Ge2 O4 K2 O6 -31.69(7) . . . . ?
K1 O4 K2 O6 80.34(8) . . . . ?
Ge1 O4 K2 O2 97.48(18) . . . 6_556 ?
Ge2 O4 K2 O2 -129.60(9) . . . 6_556 ?
K1 O4 K2 O2 -17.57(9) . . . 6_556 ?
Ge1 O4 K2 O2 -153.8(3) . . . 3_455 ?
Ge2 O4 K2 O2 -20.9(4) . . . 3_455 ?
K1 O4 K2 O2 91.1(3) . . . 3_455 ?
Ge1 O4 K2 O6 19.2(2) . . . 1_554 ?
Ge2 O4 K2 O6 152.11(9) . . . 1_554 ?
K1 O4 K2 O6 -95.87(9) . . . 1_554 ?
Ge1 O4 K2 O5 70.38(17) . . . 2_554 ?
Ge2 O4 K2 O5 -156.69(10) . . . 2_554 ?
K1 O4 K2 O5 -44.67(6) . . . 2_554 ?
Ge1 O4 K2 O5 -79.39(18) . . . 7_665 ?
Ge2 O4 K2 O5 53.54(12) . . . 7_665 ?
K1 O4 K2 O5 165.56(8) . . . 7_665 ?
Ge1 O4 K2 O4 -96.10(16) . . . 8_565 ?
Ge2 O4 K2 O4 36.82(10) . . . 8_565 ?
K1 O4 K2 O4 148.85(4) . . . 8_565 ?
Ge1 O4 K2 O3 141.01(17) . . . 6_556 ?
Ge2 O4 K2 O3 -86.07(9) . . . 6_556 ?
K1 O4 K2 O3 25.96(6) . . . 6_556 ?
Ge1 O4 K2 O3 -161.17(16) . . . 3_455 ?
Ge2 O4 K2 O3 -28.25(11) . . . 3_455 ?
K1 O4 K2 O3 83.78(7) . . . 3_455 ?
Ge1 O4 K2 Ge2 1.75(18) . . . 1_554 ?
Ge2 O4 K2 Ge2 134.68(7) . . . 1_554 ?
K1 O4 K2 Ge2 -113.30(5) . . . 1_554 ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        26.35
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         1.007
_refine_diff_density_min         -1.278
_refine_diff_density_rms         0.149
_database_code_depnum_ccdc_archive 'CCDC 995425'
#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_48xs

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Ge3  H2  K3 O10 Tb'
_chemical_formula_weight         656.01

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   Pnma

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, y+1/2, -z'
'-x, -y, -z'
'x-1/2, y, -z-1/2'
'-x-1/2, y-1/2, z-1/2'
'x, -y-1/2, z'

_cell_length_a                   13.6552(15)
_cell_length_b                   13.6541(15)
_cell_length_c                   6.0595(6)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     1129.8(2)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    2451
_cell_measurement_theta_min      6.736
_cell_measurement_theta_max      61.682

_exptl_crystal_description       rod
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    3.857
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1200
_exptl_absorpt_coefficient_mu    15.230
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.701
_exptl_absorpt_correction_T_max  0.737
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            6058
_diffrn_reflns_av_R_equivalents  0.0218
_diffrn_reflns_av_sigmaI/netI    0.0182
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_theta_min         2.98
_diffrn_reflns_theta_max         26.35
_reflns_number_total             1207
_reflns_number_gt                1145
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0192P)²+5.0151P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         1207
_refine_ls_number_parameters     85
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0195
_refine_ls_R_factor_gt           0.0186
_refine_ls_wR_factor_ref         0.0444
_refine_ls_wR_factor_gt          0.0439
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_restrained_S_all      1.064
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Tb1 Tb 0.458267(15) 0.2500 0.91117(3) 0.00588(8) Uani 1 2 d S . .
Ge1 Ge 0.24451(3) 0.2500 0.58643(8) 0.00770(12) Uani 1 2 d S . .
Ge2 Ge 0.40085(3) 0.10019(3) 0.40807(5) 0.00781(10) Uani 1 1 d . . .
O1 O 0.2961(2) 0.2500 0.8420(6) 0.0155(8) Uani 1 2 d S . .
O2 O 0.1201(3) 0.2500 0.5753(6) 0.0202(9) Uani 1 2 d S . .
O3 O 0.36799(19) -0.02630(18) 0.4125(4) 0.0160(5) Uani 1 1 d . . .
H3 H 0.4161 -0.0608 0.3835 0.024 Uiso 1 1 d R . .
O4 O 0.45888(18) 0.1270(2) 0.1650(4) 0.0155(5) Uani 1 1 d . . .
O5 O 0.28111(18) 0.14840(19) 0.4225(4) 0.0158(5) Uani 1 1 d . . .
O6 O 0.46810(18) 0.1305(2) 0.6397(4) 0.0151(5) Uani 1 1 d . . .
K1 K 0.13063(9) 0.2500 0.0829(2) 0.0256(3) Uani 1 2 d S . .
K2 K 0.13550(7) 0.01573(8) 0.41022(15) 0.0289(2) Uani 1 1 d . . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Tb1 O2 2.211(4) 6_657 ?
Tb1 O1 2.253(3) . ?
Tb1 O4 2.277(3) 1_556 ?
Tb1 O4 2.277(3) 8_566 ?
Tb1 O6 2.321(2) . ?
Tb1 O6 2.321(2) 8_565 ?
Tb1 K1 3.8080(13) 6_656 ?
Tb1 K2 3.8475(10) 2 ?
Tb1 K2 3.8475(10) 7_666 ?
Tb1 K1 3.8652(13) 6_657 ?
Tb1 K2 4.1546(12) 3_556 ?
Tb1 K2 4.1546(12) 6_657 ?
Ge1 O2 1.701(4) . ?
Ge1 O1 1.702(3) . ?
Ge1 O5 1.778(2) . ?
Ge1 O5 1.778(2) 8_565 ?
Ge1 K1 3.3863(13) 1_556 ?
Ge1 K1 3.4249(14) . ?
Ge1 K2 3.6863(10) . ?
Ge1 K2 3.6863(10) 8_565 ?
Ge2 O4 1.712(2) . ?
Ge2 O6 1.728(2) . ?
Ge2 O5 1.765(2) . ?
Ge2 O3 1.785(3) . ?
Ge2 K2 3.4427(10) 2_554 ?
Ge2 K2 3.4655(10) 2 ?
Ge2 K1 3.7460(12) 6_656 ?
Ge2 K2 3.8025(11) . ?
Ge2 K2 3.9136(11) 6_656 ?
O1 K1 2.690(4) 1_556 ?
O2 Tb1 2.211(4) 6_557 ?
O2 K1 2.988(4) . ?
O2 K1 3.079(4) 1_556 ?
O2 K2 3.3582(16) . ?
O2 K2 3.3582(16) 8_565 ?
O3 K2 3.020(3) 2 ?
O3 K2 3.047(3) 2_554 ?
O3 K1 3.224(3) 2 ?
O3 K2 3.226(3) . ?
O3 H3 0.8275 . ?
O4 Tb1 2.277(2) 1_554 ?
O4 K2 2.801(3) 2_554 ?
O4 K2 2.887(3) 6_656 ?
O4 K1 3.264(3) 6_656 ?
O5 K2 2.691(3) . ?
O5 K1 3.222(3) . ?
O6 K2 2.945(3) 2 ?
O6 K1 3.067(3) 6_656 ?
K1 O1 2.690(4) 1_554 ?
K1 O6 3.067(3) 6_556 ?
K1 O6 3.067(3) 3_455 ?
K1 O2 3.079(4) 1_554 ?
K1 O5 3.222(3) 8_565 ?
K1 O3 3.224(3) 2_554 ?
K1 O3 3.224(3) 7_665 ?
K1 O4 3.264(3) 6_556 ?
K1 O4 3.264(3) 3_455 ?
K1 Ge1 3.3863(13) 1_554 ?
K2 O4 2.801(3) 2 ?
K2 O4 2.887(3) 6_556 ?
K2 O6 2.945(3) 2_554 ?
K2 O3 3.020(3) 2_554 ?
K2 O3 3.047(3) 2 ?
K2 Ge2 3.4427(10) 2 ?
K2 Ge2 3.4655(10) 2_554 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Tb1 O1 171.41(13) 6_657 . ?
O2 Tb1 O4 88.36(9) 6_657 1_556 ?
O1 Tb1 O4 97.42(9) . 1_556 ?
O2 Tb1 O4 88.36(9) 6_657 8_566 ?
O1 Tb1 O4 97.42(9) . 8_566 ?
O4 Tb1 O4 95.01(14) 1_556 8_566 ?
O2 Tb1 O6 88.19(9) 6_657 . ?
O1 Tb1 O6 85.70(9) . . ?
O4 Tb1 O6 87.71(10) 1_556 . ?
O4 Tb1 O6 175.54(9) 8_566 . ?
O2 Tb1 O6 88.19(9) 6_657 8_565 ?
O1 Tb1 O6 85.70(9) . 8_565 ?
O4 Tb1 O6 175.54(9) 1_556 8_565 ?
O4 Tb1 O6 87.71(10) 8_566 8_565 ?
O6 Tb1 O6 89.35(14) . 8_565 ?
O2 Tb1 K1 53.95(10) 6_657 6_656 ?
O1 Tb1 K1 117.46(9) . 6_656 ?
O4 Tb1 K1 121.92(6) 1_556 6_656 ?
O4 Tb1 K1 121.92(6) 8_566 6_656 ?
O6 Tb1 K1 53.64(7) . 6_656 ?
O6 Tb1 K1 53.64(7) 8_565 6_656 ?
O2 Tb1 K2 109.427(17) 6_657 2 ?
O1 Tb1 K2 70.898(18) . 2 ?
O4 Tb1 K2 46.12(7) 1_556 2 ?
O4 Tb1 K2 134.23(7) 8_566 2 ?
O6 Tb1 K2 49.85(7) . 2 ?
O6 Tb1 K2 132.94(7) 8_565 2 ?
K1 Tb1 K2 101.800(15) 6_656 2 ?
O2 Tb1 K2 109.426(17) 6_657 7_666 ?
O1 Tb1 K2 70.898(18) . 7_666 ?
O4 Tb1 K2 134.23(7) 1_556 7_666 ?
O4 Tb1 K2 46.12(7) 8_566 7_666 ?
O6 Tb1 K2 132.94(7) . 7_666 ?
O6 Tb1 K2 49.85(7) 8_565 7_666 ?
K1 Tb1 K2 101.800(15) 6_656 7_666 ?
K2 Tb1 K2 141.13(3) 2 7_666 ?
O2 Tb1 K1 50.37(10) 6_657 6_657 ?
O1 Tb1 K1 138.23(9) . 6_657 ?
O4 Tb1 K1 57.45(7) 1_556 6_657 ?
O4 Tb1 K1 57.45(7) 8_566 6_657 ?
O6 Tb1 K1 121.80(6) . 6_657 ?
O6 Tb1 K1 121.80(6) 8_565 6_657 ?
K1 Tb1 K1 104.31(3) 6_656 6_657 ?
K2 Tb1 K1 101.761(16) 2 6_657 ?
K2 Tb1 K1 101.761(16) 7_666 6_657 ?
O2 Tb1 K2 53.72(3) 6_657 3_556 ?
O1 Tb1 K2 128.37(2) . 3_556 ?
O4 Tb1 K2 112.93(7) 1_556 3_556 ?
O4 Tb1 K2 41.77(6) 8_566 3_556 ?
O6 Tb1 K2 133.81(6) . 3_556 ?
O6 Tb1 K2 67.02(7) 8_565 3_556 ?
K1 Tb1 K2 81.069(18) 6_656 3_556 ?
K2 Tb1 K2 156.969(15) 2 3_556 ?
K2 Tb1 K2 57.87(3) 7_666 3_556 ?
K1 Tb1 K2 55.851(15) 6_657 3_556 ?
O2 Tb1 K2 53.72(3) 6_657 6_657 ?
O1 Tb1 K2 128.37(2) . 6_657 ?
O4 Tb1 K2 41.77(6) 1_556 6_657 ?
O4 Tb1 K2 112.93(7) 8_566 6_657 ?
O6 Tb1 K2 67.02(6) . 6_657 ?
O6 Tb1 K2 133.81(6) 8_565 6_657 ?
K1 Tb1 K2 81.069(18) 6_656 6_657 ?
K2 Tb1 K2 57.87(3) 2 6_657 ?
K2 Tb1 K2 156.969(15) 7_666 6_657 ?
K1 Tb1 K2 55.851(15) 6_657 6_657 ?
K2 Tb1 K2 100.70(3) 3_556 6_657 ?
O2 Ge1 O1 116.74(17) . . ?
O2 Ge1 O5 104.99(11) . . ?
O1 Ge1 O5 113.09(10) . . ?
O2 Ge1 O5 104.99(11) . 8_565 ?
O1 Ge1 O5 113.09(10) . 8_565 ?
O5 Ge1 O5 102.56(17) . 8_565 ?
O2 Ge1 K1 64.93(13) . 1_556 ?
O1 Ge1 K1 51.81(12) . 1_556 ?
O5 Ge1 K1 128.72(9) . 1_556 ?
O5 Ge1 K1 128.72(9) 8_565 1_556 ?
O2 Ge1 K1 60.72(13) . . ?
O1 Ge1 K1 177.47(12) . . ?
O5 Ge1 K1 68.27(8) . . ?
O5 Ge1 K1 68.27(8) 8_565 . ?
K1 Ge1 K1 125.66(4) 1_556 . ?
O2 Ge1 K2 65.48(4) . . ?
O1 Ge1 K2 115.53(4) . . ?
O5 Ge1 K2 43.50(9) . . ?
O5 Ge1 K2 128.95(9) 8_565 . ?
K1 Ge1 K2 94.12(2) 1_556 . ?
K1 Ge1 K2 63.803(17) . . ?
O2 Ge1 K2 65.48(4) . 8_565 ?
O1 Ge1 K2 115.53(4) . 8_565 ?
O5 Ge1 K2 128.95(9) . 8_565 ?
O5 Ge1 K2 43.50(9) 8_565 8_565 ?
K1 Ge1 K2 94.12(2) 1_556 8_565 ?
K1 Ge1 K2 63.803(17) . 8_565 ?
K2 Ge1 K2 120.40(4) . 8_565 ?
O4 Ge2 O6 113.68(12) . . ?
O4 Ge2 O5 113.05(12) . . ?
O6 Ge2 O5 111.28(11) . . ?
O4 Ge2 O3 109.66(12) . . ?
O6 Ge2 O3 110.68(13) . . ?
O5 Ge2 O3 97.32(12) . . ?
O4 Ge2 K2 53.94(9) . 2_554 ?
O6 Ge2 K2 153.98(8) . 2_554 ?
O5 Ge2 K2 94.66(8) . 2_554 ?
O3 Ge2 K2 62.10(8) . 2_554 ?
O4 Ge2 K2 156.83(9) . 2 ?
O6 Ge2 K2 58.14(9) . 2 ?
O5 Ge2 K2 89.67(9) . 2 ?
O3 Ge2 K2 60.58(8) . 2 ?
K2 Ge2 K2 122.60(3) 2_554 2 ?
O4 Ge2 K1 60.53(9) . 6_656 ?
O6 Ge2 K1 53.99(9) . 6_656 ?
O5 Ge2 K1 124.86(9) . 6_656 ?
O3 Ge2 K1 137.63(9) . 6_656 ?
K2 Ge2 K1 112.62(3) 2_554 6_656 ?
K2 Ge2 K1 110.88(3) 2 6_656 ?
O4 Ge2 K2 120.59(9) . . ?
O6 Ge2 K2 125.20(9) . . ?
O5 Ge2 K2 39.66(9) . . ?
O3 Ge2 K2 57.78(9) . . ?
K2 Ge2 K2 74.11(2) 2_554 . ?
K2 Ge2 K2 73.86(2) 2 . ?
K1 Ge2 K2 164.52(2) 6_656 . ?
O4 Ge2 K2 42.29(9) . 6_656 ?
O6 Ge2 K2 92.05(8) . 6_656 ?
O5 Ge2 K2 153.23(8) . 6_656 ?
O3 Ge2 K2 85.88(8) . 6_656 ?
K2 Ge2 K2 63.30(3) 2_554 6_656 ?
K2 Ge2 K2 114.542(18) 2 6_656 ?
K1 Ge2 K2 58.83(2) 6_656 6_656 ?
K2 Ge2 K2 133.83(2) . 6_656 ?
Ge1 O1 Tb1 125.19(18) . . ?
Ge1 O1 K1 98.38(14) . 1_556 ?
Tb1 O1 K1 136.43(15) . 1_556 ?
Ge1 O2 Tb1 175.6(2) . 6_557 ?
Ge1 O2 K1 89.51(15) . . ?
Tb1 O2 K1 94.89(13) 6_557 . ?
Ge1 O2 K1 85.05(14) . 1_556 ?
Tb1 O2 K1 90.56(12) 6_557 1_556 ?
K1 O2 K1 174.55(15) . 1_556 ?
Ge1 O2 K2 87.08(7) . . ?
Tb1 O2 K2 94.23(7) 6_557 . ?
K1 O2 K2 72.51(6) . . ?
K1 O2 K2 107.14(6) 1_556 . ?
Ge1 O2 K2 87.08(7) . 8_565 ?
Tb1 O2 K2 94.23(7) 6_557 8_565 ?
K1 O2 K2 72.51(6) . 8_565 ?
K1 O2 K2 107.14(6) 1_556 8_565 ?
K2 O2 K2 144.55(13) . 8_565 ?
Ge2 O3 K2 88.44(10) . 2 ?
Ge2 O3 K2 86.73(9) . 2_554 ?
K2 O3 K2 174.26(11) 2 2_554 ?
Ge2 O3 K1 156.95(13) . 2 ?
K2 O3 K1 74.08(6) 2 2 ?
K2 O3 K1 111.39(8) 2_554 2 ?
Ge2 O3 K2 94.31(10) . . ?
K2 O3 K2 88.87(7) 2 . ?
K2 O3 K2 88.39(7) 2_554 . ?
K1 O3 K2 100.11(7) 2 . ?
Ge2 O3 H3 110.3 . . ?
K2 O3 H3 104.6 2 . ?
K2 O3 H3 80.0 2_554 . ?
K1 O3 H3 61.6 2 . ?
K2 O3 H3 151.9 . . ?
Ge2 O4 Tb1 137.49(14) . 1_554 ?
Ge2 O4 K2 96.45(11) . 2_554 ?
Tb1 O4 K2 98.00(9) 1_554 2_554 ?
Ge2 O4 K2 114.19(12) . 6_656 ?
Tb1 O4 K2 106.53(9) 1_554 6_656 ?
K2 O4 K2 86.04(8) 2_554 6_656 ?
Ge2 O4 K1 92.29(10) . 6_656 ?
Tb1 O4 K1 86.53(8) 1_554 6_656 ?
K2 O4 K1 161.20(10) 2_554 6_656 ?
K2 O4 K1 75.19(6) 6_656 6_656 ?
Ge2 O5 Ge1 125.39(14) . . ?
Ge2 O5 K2 115.60(12) . . ?
Ge1 O5 K2 109.45(11) . . ?
Ge2 O5 K1 136.04(12) . . ?
Ge1 O5 K1 80.89(9) . . ?
K2 O5 K1 78.52(7) . . ?
Ge2 O6 Tb1 135.51(13) . . ?
Ge2 O6 K2 91.98(10) . 2 ?
Tb1 O6 K2 93.12(8) . 2 ?
Ge2 O6 K1 98.90(11) . 6_656 ?
Tb1 O6 K1 88.82(8) . 6_656 ?
K2 O6 K1 162.36(10) 2 6_656 ?
O1 K1 O2 125.62(11) 1_554 . ?
O1 K1 O6 111.67(8) 1_554 6_556 ?
O2 K1 O6 113.85(8) . 6_556 ?
O1 K1 O6 111.67(8) 1_554 3_455 ?
O2 K1 O6 113.85(8) . 3_455 ?
O6 K1 O6 64.29(10) 6_556 3_455 ?
O1 K1 O2 59.83(10) 1_554 1_554 ?
O2 K1 O2 174.55(15) . 1_554 ?
O6 K1 O2 61.76(7) 6_556 1_554 ?
O6 K1 O2 61.76(7) 3_455 1_554 ?
O1 K1 O5 79.09(8) 1_554 8_565 ?
O2 K1 O5 52.61(8) . 8_565 ?
O6 K1 O5 166.26(7) 6_556 8_565 ?
O6 K1 O5 120.88(7) 3_455 8_565 ?
O2 K1 O5 131.90(8) 1_554 8_565 ?
O1 K1 O5 79.09(8) 1_554 . ?
O2 K1 O5 52.61(8) . . ?
O6 K1 O5 120.88(7) 6_556 . ?
O6 K1 O5 166.26(7) 3_455 . ?
O2 K1 O5 131.90(8) 1_554 . ?
O5 K1 O5 51.00(9) 8_565 . ?
O1 K1 O3 79.71(5) 1_554 2_554 ?
O2 K1 O3 108.67(5) . 2_554 ?
O6 K1 O3 50.17(7) 6_556 2_554 ?
O6 K1 O3 111.56(7) 3_455 2_554 ?
O2 K1 O3 71.37(5) 1_554 2_554 ?
O5 K1 O3 127.49(7) 8_565 2_554 ?
O5 K1 O3 78.05(6) . 2_554 ?
O1 K1 O3 79.71(5) 1_554 7_665 ?
O2 K1 O3 108.67(5) . 7_665 ?
O6 K1 O3 111.56(7) 6_556 7_665 ?
O6 K1 O3 50.17(7) 3_455 7_665 ?
O2 K1 O3 71.37(5) 1_554 7_665 ?
O5 K1 O3 78.05(6) 8_565 7_665 ?
O5 K1 O3 127.49(7) . 7_665 ?
O3 K1 O3 142.65(10) 2_554 7_665 ?
O1 K1 O4 149.04(5) 1_554 6_556 ?
O2 K1 O4 59.85(7) . 6_556 ?
O6 K1 O4 54.00(7) 6_556 6_556 ?
O6 K1 O4 87.68(7) 3_455 6_556 ?
O2 K1 O4 115.72(8) 1_554 6_556 ?
O5 K1 O4 112.38(7) 8_565 6_556 ?
O5 K1 O4 86.43(7) . 6_556 ?
O3 K1 O4 70.53(7) 2_554 6_556 ?
O3 K1 O4 129.89(7) 7_665 6_556 ?
O1 K1 O4 149.04(5) 1_554 3_455 ?
O2 K1 O4 59.85(7) . 3_455 ?
O6 K1 O4 87.68(7) 6_556 3_455 ?
O6 K1 O4 54.00(7) 3_455 3_455 ?
O2 K1 O4 115.72(8) 1_554 3_455 ?
O5 K1 O4 86.43(7) 8_565 3_455 ?
O5 K1 O4 112.38(7) . 3_455 ?
O3 K1 O4 129.89(7) 2_554 3_455 ?
O3 K1 O4 70.53(7) 7_665 3_455 ?
O4 K1 O4 61.92(9) 6_556 3_455 ?
O1 K1 Ge1 29.81(7) 1_554 1_554 ?
O2 K1 Ge1 155.43(9) . 1_554 ?
O6 K1 Ge1 86.66(5) 6_556 1_554 ?
O6 K1 Ge1 86.66(5) 3_455 1_554 ?
O2 K1 Ge1 30.02(7) 1_554 1_554 ?
O5 K1 Ge1 105.93(6) 8_565 1_554 ?
O5 K1 Ge1 105.93(6) . 1_554 ?
O3 K1 Ge1 73.32(5) 2_554 1_554 ?
O3 K1 Ge1 73.32(5) 7_665 1_554 ?
O4 K1 Ge1 138.23(5) 6_556 1_554 ?
O4 K1 Ge1 138.23(5) 3_455 1_554 ?
O5 K2 O4 142.50(8) . 2 ?
O5 K2 O4 105.50(8) . 6_556 ?
O4 K2 O4 93.96(8) 2 6_556 ?
O5 K2 O6 145.76(8) . 2_554 ?
O4 K2 O6 67.29(7) 2 2_554 ?
O4 K2 O6 82.40(7) 6_556 2_554 ?
O5 K2 O3 90.40(8) . 2_554 ?
O4 K2 O3 125.21(7) 2 2_554 ?
O4 K2 O3 78.69(8) 6_556 2_554 ?
O6 K2 O3 57.93(7) 2_554 2_554 ?
O5 K2 O3 87.26(7) . 2 ?
O4 K2 O3 58.34(7) 2 2 ?
O4 K2 O3 96.88(8) 6_556 2 ?
O6 K2 O3 125.48(7) 2_554 2 ?
O3 K2 O3 174.26(11) 2_554 2 ?
O5 K2 O3 52.59(7) . . ?
O4 K2 O3 109.07(7) 2 . ?
O4 K2 O3 156.41(8) 6_556 . ?
O6 K2 O3 110.76(7) 2_554 . ?
O3 K2 O3 91.62(7) 2_554 . ?
O3 K2 O3 91.12(7) 2 . ?
O5 K2 O2 52.90(8) . . ?
O4 K2 O2 118.02(9) 2 . ?
O4 K2 O2 59.55(8) 6_556 . ?
O6 K2 O2 141.39(9) 2_554 . ?
O3 K2 O2 104.54(8) 2_554 . ?
O3 K2 O2 69.90(8) 2 . ?
O3 K2 O2 103.29(8) . . ?
O5 K2 Ge2 113.07(6) . 2 ?
O4 K2 Ge2 29.62(5) 2 2 ?
O4 K2 Ge2 105.07(6) 6_556 2 ?
O6 K2 Ge2 96.13(5) 2_554 2 ?
O3 K2 Ge2 153.49(6) 2_554 2 ?
O3 K2 Ge2 31.17(5) 2 2 ?
O3 K2 Ge2 93.23(5) . 2 ?
O2 K2 Ge2 99.66(7) . 2 ?
O5 K2 Ge2 115.94(6) . 2_554 ?
O4 K2 Ge2 95.76(6) 2 2_554 ?
O4 K2 Ge2 88.98(5) 6_556 2_554 ?
O6 K2 Ge2 29.88(5) 2_554 2_554 ?
O3 K2 Ge2 30.98(5) 2_554 2_554 ?
O3 K2 Ge2 153.68(6) 2 2_554 ?
O3 K2 Ge2 93.64(5) . 2_554 ?
O2 K2 Ge2 133.44(7) . 2_554 ?
Ge2 K2 Ge2 122.60(3) 2 2_554 ?
O5 K2 Ge1 27.05(5) . . ?
O4 K2 Ge1 129.06(6) 2 . ?
O4 K2 Ge1 85.77(6) 6_556 . ?
O6 K2 Ge1 160.64(6) 2_554 . ?
O3 K2 Ge1 104.73(5) 2_554 . ?
O3 K2 Ge1 71.09(5) 2 . ?
O3 K2 Ge1 75.86(5) . . ?
O2 K2 Ge1 27.43(6) . . ?
Ge2 K2 Ge1 101.73(2) 2 . ?
Ge2 K2 Ge1 135.11(3) 2_554 . ?
O5 K2 K1 57.01(6) . . ?
O4 K2 K1 150.90(7) 2 . ?
O4 K2 K1 56.96(6) 6_556 . ?
O6 K2 K1 105.92(6) 2_554 . ?
O3 K2 K1 55.45(5) 2_554 . ?
O3 K2 K1 119.06(6) 2 . ?
O3 K2 K1 99.83(5) . . ?
O2 K2 K1 49.19(6) . . ?
Ge2 K2 K1 148.19(4) 2 . ?
Ge2 K2 K1 85.58(3) 2_554 . ?
Ge1 K2 K1 54.72(2) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Ge1 O1 Tb1 180.0 . . . . ?
O5 Ge1 O1 Tb1 58.01(10) . . . . ?
O5 Ge1 O1 Tb1 -58.01(10) 8_565 . . . ?
K1 Ge1 O1 Tb1 180.0 1_556 . . . ?
K1 Ge1 O1 Tb1 180.000(9) . . . . ?
K2 Ge1 O1 Tb1 105.92(6) . . . . ?
K2 Ge1 O1 Tb1 -105.92(6) 8_565 . . . ?
O2 Ge1 O1 K1 0.0 . . . 1_556 ?
O5 Ge1 O1 K1 -121.99(10) . . . 1_556 ?
O5 Ge1 O1 K1 121.99(10) 8_565 . . 1_556 ?
K1 Ge1 O1 K1 0.000(9) . . . 1_556 ?
K2 Ge1 O1 K1 -74.08(6) . . . 1_556 ?
K2 Ge1 O1 K1 74.08(6) 8_565 . . 1_556 ?
O2 Tb1 O1 Ge1 0.000(2) 6_657 . . . ?
O4 Tb1 O1 Ge1 -131.96(7) 1_556 . . . ?
O4 Tb1 O1 Ge1 131.96(7) 8_566 . . . ?
O6 Tb1 O1 Ge1 -44.84(7) . . . . ?
O6 Tb1 O1 Ge1 44.84(7) 8_565 . . . ?
K1 Tb1 O1 Ge1 0.0 6_656 . . . ?
K2 Tb1 O1 Ge1 -93.67(3) 2 . . . ?
K2 Tb1 O1 Ge1 93.67(3) 7_666 . . . ?
K1 Tb1 O1 Ge1 180.0 6_657 . . . ?
K2 Tb1 O1 Ge1 100.85(7) 3_556 . . . ?
K2 Tb1 O1 Ge1 -100.85(7) 6_657 . . . ?
O2 Tb1 O1 K1 180.000(2) 6_657 . . 1_556 ?
O4 Tb1 O1 K1 48.04(7) 1_556 . . 1_556 ?
O4 Tb1 O1 K1 -48.04(7) 8_566 . . 1_556 ?
O6 Tb1 O1 K1 135.16(7) . . . 1_556 ?
O6 Tb1 O1 K1 -135.16(7) 8_565 . . 1_556 ?
K1 Tb1 O1 K1 180.0 6_656 . . 1_556 ?
K2 Tb1 O1 K1 86.33(3) 2 . . 1_556 ?
K2 Tb1 O1 K1 -86.33(3) 7_666 . . 1_556 ?
K1 Tb1 O1 K1 0.0 6_657 . . 1_556 ?
K2 Tb1 O1 K1 -79.14(7) 3_556 . . 1_556 ?
K2 Tb1 O1 K1 79.15(7) 6_657 . . 1_556 ?
O1 Ge1 O2 Tb1 0.000(4) . . . 6_557 ?
O5 Ge1 O2 Tb1 126.13(9) . . . 6_557 ?
O5 Ge1 O2 Tb1 -126.13(9) 8_565 . . 6_557 ?
K1 Ge1 O2 Tb1 0.000(4) 1_556 . . 6_557 ?
K1 Ge1 O2 Tb1 180.000(4) . . . 6_557 ?
K2 Ge1 O2 Tb1 107.49(6) . . . 6_557 ?
K2 Ge1 O2 Tb1 -107.49(6) 8_565 . . 6_557 ?
O1 Ge1 O2 K1 180.0 . . . . ?
O5 Ge1 O2 K1 -53.87(9) . . . . ?
O5 Ge1 O2 K1 53.87(9) 8_565 . . . ?
K1 Ge1 O2 K1 180.0 1_556 . . . ?
K2 Ge1 O2 K1 -72.51(6) . . . . ?
K2 Ge1 O2 K1 72.51(6) 8_565 . . . ?
O1 Ge1 O2 K1 0.0 . . . 1_556 ?
O5 Ge1 O2 K1 126.13(9) . . . 1_556 ?
O5 Ge1 O2 K1 -126.13(9) 8_565 . . 1_556 ?
K1 Ge1 O2 K1 180.0 . . . 1_556 ?
K2 Ge1 O2 K1 107.49(6) . . . 1_556 ?
K2 Ge1 O2 K1 -107.49(6) 8_565 . . 1_556 ?
O1 Ge1 O2 K2 -107.49(6) . . . . ?
O5 Ge1 O2 K2 18.64(12) . . . . ?
O5 Ge1 O2 K2 126.38(10) 8_565 . . . ?
K1 Ge1 O2 K2 -107.49(6) 1_556 . . . ?
K1 Ge1 O2 K2 72.51(6) . . . . ?
K2 Ge1 O2 K2 145.02(11) 8_565 . . . ?
O1 Ge1 O2 K2 107.49(6) . . . 8_565 ?
O5 Ge1 O2 K2 -126.38(10) . . . 8_565 ?
O5 Ge1 O2 K2 -18.64(12) 8_565 . . 8_565 ?
K1 Ge1 O2 K2 107.49(6) 1_556 . . 8_565 ?
K1 Ge1 O2 K2 -72.51(6) . . . 8_565 ?
K2 Ge1 O2 K2 -145.02(11) . . . 8_565 ?
O4 Ge2 O3 K2 156.82(10) . . . 2 ?
O6 Ge2 O3 K2 30.61(12) . . . 2 ?
O5 Ge2 O3 K2 -85.47(10) . . . 2 ?
K2 Ge2 O3 K2 -176.88(10) 2_554 . . 2 ?
K1 Ge2 O3 K2 89.37(11) 6_656 . . 2 ?
K2 Ge2 O3 K2 -88.75(7) . . . 2 ?
K2 Ge2 O3 K2 121.25(5) 6_656 . . 2 ?
O4 Ge2 O3 K2 -26.30(12) . . . 2_554 ?
O6 Ge2 O3 K2 -152.50(9) . . . 2_554 ?
O5 Ge2 O3 K2 91.42(10) . . . 2_554 ?
K2 Ge2 O3 K2 176.88(10) 2 . . 2_554 ?
K1 Ge2 O3 K2 -93.75(11) 6_656 . . 2_554 ?
K2 Ge2 O3 K2 88.13(7) . . . 2_554 ?
K2 Ge2 O3 K2 -61.87(5) 6_656 . . 2_554 ?
O4 Ge2 O3 K1 116.7(3) . . . 2 ?
O6 Ge2 O3 K1 -9.5(4) . . . 2 ?
O5 Ge2 O3 K1 -125.6(3) . . . 2 ?
K2 Ge2 O3 K1 143.0(4) 2_554 . . 2 ?
K2 Ge2 O3 K1 -40.1(3) 2 . . 2 ?
K1 Ge2 O3 K1 49.3(4) 6_656 . . 2 ?
K2 Ge2 O3 K1 -128.8(3) . . . 2 ?
K2 Ge2 O3 K1 81.2(3) 6_656 . . 2 ?
O4 Ge2 O3 K2 -114.43(10) . . . . ?
O6 Ge2 O3 K2 119.36(10) . . . . ?
O5 Ge2 O3 K2 3.28(10) . . . . ?
K2 Ge2 O3 K2 -88.13(7) 2_554 . . . ?
K2 Ge2 O3 K2 88.75(7) 2 . . . ?
K1 Ge2 O3 K2 178.12(5) 6_656 . . . ?
K2 Ge2 O3 K2 -150.00(6) 6_656 . . . ?
O6 Ge2 O4 Tb1 -97.3(2) . . . 1_554 ?
O5 Ge2 O4 Tb1 30.9(2) . . . 1_554 ?
O3 Ge2 O4 Tb1 138.26(19) . . . 1_554 ?
K2 Ge2 O4 Tb1 109.3(2) 2_554 . . 1_554 ?
K2 Ge2 O4 Tb1 -161.13(8) 2 . . 1_554 ?
K1 Ge2 O4 Tb1 -87.4(2) 6_656 . . 1_554 ?
K2 Ge2 O4 Tb1 74.8(2) . . . 1_554 ?
K2 Ge2 O4 Tb1 -162.2(3) 6_656 . . 1_554 ?
O6 Ge2 O4 K2 153.45(10) . . . 2_554 ?
O5 Ge2 O4 K2 -78.43(12) . . . 2_554 ?
O3 Ge2 O4 K2 28.97(13) . . . 2_554 ?
K2 Ge2 O4 K2 89.6(2) 2 . . 2_554 ?
K1 Ge2 O4 K2 163.33(11) 6_656 . . 2_554 ?
K2 Ge2 O4 K2 -34.52(12) . . . 2_554 ?
K2 Ge2 O4 K2 88.54(12) 6_656 . . 2_554 ?
O6 Ge2 O4 K2 64.91(16) . . . 6_656 ?
O5 Ge2 O4 K2 -166.97(11) . . . 6_656 ?
O3 Ge2 O4 K2 -59.58(15) . . . 6_656 ?
K2 Ge2 O4 K2 -88.54(12) 2_554 . . 6_656 ?
K2 Ge2 O4 K2 1.0(3) 2 . . 6_656 ?
K1 Ge2 O4 K2 74.79(10) 6_656 . . 6_656 ?
K2 Ge2 O4 K2 -123.06(9) . . . 6_656 ?
O6 Ge2 O4 K1 -9.88(13) . . . 6_656 ?
O5 Ge2 O4 K1 118.24(10) . . . 6_656 ?
O3 Ge2 O4 K1 -134.37(10) . . . 6_656 ?
K2 Ge2 O4 K1 -163.33(11) 2_554 . . 6_656 ?
K2 Ge2 O4 K1 -73.8(2) 2 . . 6_656 ?
K2 Ge2 O4 K1 162.15(3) . . . 6_656 ?
K2 Ge2 O4 K1 -74.79(10) 6_656 . . 6_656 ?
O4 Ge2 O5 Ge1 -106.82(19) . . . . ?
O6 Ge2 O5 Ge1 22.5(2) . . . . ?
O3 Ge2 O5 Ge1 138.14(18) . . . . ?
K2 Ge2 O5 Ge1 -159.43(16) 2_554 . . . ?
K2 Ge2 O5 Ge1 77.88(17) 2 . . . ?
K1 Ge2 O5 Ge1 -37.6(2) 6_656 . . . ?
K2 Ge2 O5 Ge1 142.5(3) . . . . ?
K2 Ge2 O5 Ge1 -126.49(14) 6_656 . . . ?
O4 Ge2 O5 K2 110.69(14) . . . . ?
O6 Ge2 O5 K2 -119.95(13) . . . . ?
O3 Ge2 O5 K2 -4.35(14) . . . . ?
K2 Ge2 O5 K2 58.07(10) 2_554 . . . ?
K2 Ge2 O5 K2 -64.62(10) 2 . . . ?
K1 Ge2 O5 K2 179.89(5) 6_656 . . . ?
K2 Ge2 O5 K2 91.0(2) 6_656 . . . ?
O4 Ge2 O5 K1 10.4(2) . . . . ?
O6 Ge2 O5 K1 139.73(16) . . . . ?
O3 Ge2 O5 K1 -104.67(17) . . . . ?
K2 Ge2 O5 K1 -42.24(16) 2_554 . . . ?
K2 Ge2 O5 K1 -164.93(15) 2 . . . ?
K1 Ge2 O5 K1 79.57(17) 6_656 . . . ?
K2 Ge2 O5 K1 -100.31(19) . . . . ?
K2 Ge2 O5 K1 -9.3(3) 6_656 . . . ?
O2 Ge1 O5 Ge2 -169.37(18) . . . . ?
O1 Ge1 O5 Ge2 -41.0(2) . . . . ?
O5 Ge1 O5 Ge2 81.1(2) 8_565 . . . ?
K1 Ge1 O5 Ge2 -99.71(17) 1_556 . . . ?
K1 Ge1 O5 Ge2 141.3(2) . . . . ?
K2 Ge1 O5 Ge2 -144.4(2) . . . . ?
K2 Ge1 O5 Ge2 120.26(14) 8_565 . . . ?
O2 Ge1 O5 K2 -24.98(15) . . . . ?
O1 Ge1 O5 K2 103.37(14) . . . . ?
O5 Ge1 O5 K2 -134.50(8) 8_565 . . . ?
K1 Ge1 O5 K2 44.68(14) 1_556 . . . ?
K1 Ge1 O5 K2 -74.31(9) . . . . ?
K2 Ge1 O5 K2 -95.35(12) 8_565 . . . ?
O2 Ge1 O5 K1 49.33(12) . . . . ?
O1 Ge1 O5 K1 177.69(11) . . . . ?
O5 Ge1 O5 K1 -60.19(12) 8_565 . . . ?
K1 Ge1 O5 K1 119.00(8) 1_556 . . . ?
K2 Ge1 O5 K1 74.31(9) . . . . ?
K2 Ge1 O5 K1 -21.04(11) 8_565 . . . ?
O4 Ge2 O6 Tb1 108.1(2) . . . . ?
O5 Ge2 O6 Tb1 -20.9(2) . . . . ?
O3 Ge2 O6 Tb1 -127.96(19) . . . . ?
K2 Ge2 O6 Tb1 163.57(7) 2_554 . . . ?
K2 Ge2 O6 Tb1 -96.48(19) 2 . . . ?
K1 Ge2 O6 Tb1 97.5(2) 6_656 . . . ?
K2 Ge2 O6 Tb1 -63.5(2) . . . . ?
K2 Ge2 O6 Tb1 145.67(18) 6_656 . . . ?
O4 Ge2 O6 K2 -155.42(10) . . . 2 ?
O5 Ge2 O6 K2 75.56(12) . . . 2 ?
O3 Ge2 O6 K2 -31.48(12) . . . 2 ?
K2 Ge2 O6 K2 -99.96(19) 2_554 . . 2 ?
K1 Ge2 O6 K2 -166.06(11) 6_656 . . 2 ?
K2 Ge2 O6 K2 32.98(12) . . . 2 ?
K2 Ge2 O6 K2 -117.85(5) 6_656 . . 2 ?
O4 Ge2 O6 K1 10.64(14) . . . 6_656 ?
O5 Ge2 O6 K1 -118.38(11) . . . 6_656 ?
O3 Ge2 O6 K1 134.58(10) . . . 6_656 ?
K2 Ge2 O6 K1 66.1(2) 2_554 . . 6_656 ?
K2 Ge2 O6 K1 166.06(11) 2 . . 6_656 ?
K2 Ge2 O6 K1 -160.96(3) . . . 6_656 ?
K2 Ge2 O6 K1 48.22(7) 6_656 . . 6_656 ?
O2 Tb1 O6 Ge2 -146.5(2) 6_657 . . . ?
O1 Tb1 O6 Ge2 27.5(2) . . . . ?
O4 Tb1 O6 Ge2 125.1(2) 1_556 . . . ?
O4 Tb1 O6 Ge2 -107.1(11) 8_566 . . . ?
O6 Tb1 O6 Ge2 -58.3(2) 8_565 . . . ?
K1 Tb1 O6 Ge2 -101.5(2) 6_656 . . . ?
K2 Tb1 O6 Ge2 96.0(2) 2 . . . ?
K2 Tb1 O6 Ge2 -31.3(2) 7_666 . . . ?
K1 Tb1 O6 Ge2 173.93(16) 6_657 . . . ?
K2 Tb1 O6 Ge2 -114.76(17) 3_556 . . . ?
K2 Tb1 O6 Ge2 162.6(2) 6_657 . . . ?
O2 Tb1 O6 K2 117.52(9) 6_657 . . 2 ?
O1 Tb1 O6 K2 -68.53(8) . . . 2 ?
O4 Tb1 O6 K2 29.09(8) 1_556 . . 2 ?
O4 Tb1 O6 K2 156.8(11) 8_566 . . 2 ?
O6 Tb1 O6 K2 -154.27(4) 8_565 . . 2 ?
K1 Tb1 O6 K2 162.45(10) 6_656 . . 2 ?
K2 Tb1 O6 K2 -127.32(7) 7_666 . . 2 ?
K1 Tb1 O6 K2 77.92(8) 6_657 . . 2 ?
K2 Tb1 O6 K2 149.22(4) 3_556 . . 2 ?
K2 Tb1 O6 K2 66.55(6) 6_657 . . 2 ?
O2 Tb1 O6 K1 -44.93(8) 6_657 . . 6_656 ?
O1 Tb1 O6 K1 129.02(8) . . . 6_656 ?
O4 Tb1 O6 K1 -133.36(8) 1_556 . . 6_656 ?
O4 Tb1 O6 K1 -5.6(12) 8_566 . . 6_656 ?
O6 Tb1 O6 K1 43.28(10) 8_565 . . 6_656 ?
K2 Tb1 O6 K1 -162.45(10) 2 . . 6_656 ?
K2 Tb1 O6 K1 70.23(9) 7_666 . . 6_656 ?
K1 Tb1 O6 K1 -84.53(7) 6_657 . . 6_656 ?
K2 Tb1 O6 K1 -13.22(11) 3_556 . . 6_656 ?
K2 Tb1 O6 K1 -95.90(6) 6_657 . . 6_656 ?
Ge1 O2 K1 O1 0.0 . . . 1_554 ?
Tb1 O2 K1 O1 180.0 6_557 . . 1_554 ?
K1 O2 K1 O1 0.000(3) 1_556 . . 1_554 ?
K2 O2 K1 O1 -87.10(5) . . . 1_554 ?
K2 O2 K1 O1 87.10(5) 8_565 . . 1_554 ?
Ge1 O2 K1 O6 144.43(6) . . . 6_556 ?
Tb1 O2 K1 O6 -35.57(6) 6_557 . . 6_556 ?
K1 O2 K1 O6 144.43(6) 1_556 . . 6_556 ?
K2 O2 K1 O6 57.33(8) . . . 6_556 ?
K2 O2 K1 O6 -128.47(7) 8_565 . . 6_556 ?
Ge1 O2 K1 O6 -144.43(6) . . . 3_455 ?
Tb1 O2 K1 O6 35.57(6) 6_557 . . 3_455 ?
K1 O2 K1 O6 -144.43(6) 1_556 . . 3_455 ?
K2 O2 K1 O6 128.47(7) . . . 3_455 ?
K2 O2 K1 O6 -57.33(8) 8_565 . . 3_455 ?
Ge1 O2 K1 O2 180.000(2) . . . 1_554 ?
Tb1 O2 K1 O2 0.000(1) 6_557 . . 1_554 ?
K1 O2 K1 O2 180.000(4) 1_556 . . 1_554 ?
K2 O2 K1 O2 92.90(5) . . . 1_554 ?
K2 O2 K1 O2 -92.90(5) 8_565 . . 1_554 ?
Ge1 O2 K1 O5 -32.81(6) . . . 8_565 ?
Tb1 O2 K1 O5 147.19(6) 6_557 . . 8_565 ?
K1 O2 K1 O5 -32.81(7) 1_556 . . 8_565 ?
K2 O2 K1 O5 -119.91(9) . . . 8_565 ?
K2 O2 K1 O5 54.29(6) 8_565 . . 8_565 ?
Ge1 O2 K1 O5 32.81(6) . . . . ?
Tb1 O2 K1 O5 -147.19(6) 6_557 . . . ?
K1 O2 K1 O5 32.81(7) 1_556 . . . ?
K2 O2 K1 O5 -54.29(6) . . . . ?
K2 O2 K1 O5 119.91(9) 8_565 . . . ?
Ge1 O2 K1 O3 90.58(6) . . . 2_554 ?
Tb1 O2 K1 O3 -89.42(6) 6_557 . . 2_554 ?
K1 O2 K1 O3 90.58(6) 1_556 . . 2_554 ?
K2 O2 K1 O3 3.48(9) . . . 2_554 ?
K2 O2 K1 O3 177.68(7) 8_565 . . 2_554 ?
Ge1 O2 K1 O3 -90.58(6) . . . 7_665 ?
Tb1 O2 K1 O3 89.42(6) 6_557 . . 7_665 ?
K1 O2 K1 O3 -90.58(6) 1_556 . . 7_665 ?
K2 O2 K1 O3 -177.68(7) . . . 7_665 ?
K2 O2 K1 O3 -3.48(9) 8_565 . . 7_665 ?
Ge1 O2 K1 O4 143.50(6) . . . 6_556 ?
Tb1 O2 K1 O4 -36.50(6) 6_557 . . 6_556 ?
K1 O2 K1 O4 143.50(6) 1_556 . . 6_556 ?
K2 O2 K1 O4 56.40(6) . . . 6_556 ?
K2 O2 K1 O4 -129.40(9) 8_565 . . 6_556 ?
Ge1 O2 K1 O4 -143.50(6) . . . 3_455 ?
Tb1 O2 K1 O4 36.50(6) 6_557 . . 3_455 ?
K1 O2 K1 O4 -143.50(6) 1_556 . . 3_455 ?
K2 O2 K1 O4 129.40(9) . . . 3_455 ?
K2 O2 K1 O4 -56.40(6) 8_565 . . 3_455 ?
Ge1 O2 K1 Ge1 0.0 . . . 1_554 ?
Tb1 O2 K1 Ge1 180.0 6_557 . . 1_554 ?
K1 O2 K1 Ge1 0.000(3) 1_556 . . 1_554 ?
K2 O2 K1 Ge1 -87.10(5) . . . 1_554 ?
K2 O2 K1 Ge1 87.10(5) 8_565 . . 1_554 ?
Ge2 O5 K1 O1 -11.06(16) . . . 1_554 ?
Ge1 O5 K1 O1 121.69(9) . . . 1_554 ?
K2 O5 K1 O1 -126.18(6) . . . 1_554 ?
Ge2 O5 K1 O2 -164.4(2) . . . . ?
Ge1 O5 K1 O2 -31.66(7) . . . . ?
K2 O5 K1 O2 80.47(8) . . . . ?
Ge2 O5 K1 O6 97.79(18) . . . 6_556 ?
Ge1 O5 K1 O6 -129.47(9) . . . 6_556 ?
K2 O5 K1 O6 -17.34(10) . . . 6_556 ?
Ge2 O5 K1 O6 -153.7(2) . . . 3_455 ?
Ge1 O5 K1 O6 -21.0(4) . . . 3_455 ?
K2 O5 K1 O6 91.2(3) . . . 3_455 ?
Ge2 O5 K1 O2 19.6(2) . . . 1_554 ?
Ge1 O5 K1 O2 152.30(8) . . . 1_554 ?
K2 O5 K1 O2 -95.57(9) . . . 1_554 ?
Ge2 O5 K1 O5 -95.78(17) . . . 8_565 ?
Ge1 O5 K1 O5 36.96(10) . . . 8_565 ?
K2 O5 K1 O5 149.09(4) . . . 8_565 ?
Ge2 O5 K1 O3 70.60(17) . . . 2_554 ?
Ge1 O5 K1 O3 -156.65(10) . . . 2_554 ?
K2 O5 K1 O3 -44.53(7) . . . 2_554 ?
Ge2 O5 K1 O3 -78.91(19) . . . 7_665 ?
Ge1 O5 K1 O3 53.84(13) . . . 7_665 ?
K2 O5 K1 O3 165.97(8) . . . 7_665 ?
Ge2 O5 K1 O4 141.45(18) . . . 6_556 ?
Ge1 O5 K1 O4 -85.81(9) . . . 6_556 ?
K2 O5 K1 O4 26.32(7) . . . 6_556 ?
Ge2 O5 K1 O4 -160.95(16) . . . 3_455 ?
Ge1 O5 K1 O4 -28.21(11) . . . 3_455 ?
K2 O5 K1 O4 83.92(8) . . . 3_455 ?
Ge2 O5 K1 Ge1 2.05(18) . . . 1_554 ?
Ge1 O5 K1 Ge1 134.79(7) . . . 1_554 ?
K2 O5 K1 Ge1 -113.08(5) . . . 1_554 ?
Ge2 O5 K2 O4 74.27(18) . . . 2 ?
Ge1 O5 K2 O4 -73.97(18) . . . 2 ?
K1 O5 K2 O4 -149.90(12) . . . 2 ?
Ge2 O5 K2 O4 -167.11(11) . . . 6_556 ?
Ge1 O5 K2 O4 44.66(13) . . . 6_556 ?
K1 O5 K2 O4 -31.28(8) . . . 6_556 ?
Ge2 O5 K2 O6 -67.7(2) . . . 2_554 ?
Ge1 O5 K2 O6 144.07(13) . . . 2_554 ?
K1 O5 K2 O6 68.13(15) . . . 2_554 ?
Ge2 O5 K2 O3 -88.73(13) . . . 2_554 ?
Ge1 O5 K2 O3 123.03(12) . . . 2_554 ?
K1 O5 K2 O3 47.10(7) . . . 2_554 ?
Ge2 O5 K2 O3 96.52(13) . . . 2 ?
Ge1 O5 K2 O3 -51.72(12) . . . 2 ?
K1 O5 K2 O3 -127.66(7) . . . 2 ?
Ge2 O5 K2 O3 3.01(10) . . . . ?
Ge1 O5 K2 O3 -145.23(15) . . . . ?
K1 O5 K2 O3 138.83(9) . . . . ?
Ge2 O5 K2 O2 163.25(17) . . . . ?
Ge1 O5 K2 O2 15.01(10) . . . . ?
K1 O5 K2 O2 -60.92(9) . . . . ?
Ge2 O5 K2 Ge2 78.61(12) . . . 2 ?
Ge1 O5 K2 Ge2 -69.63(12) . . . 2 ?
K1 O5 K2 Ge2 -145.57(5) . . . 2 ?
Ge2 O5 K2 Ge2 -70.54(13) . . . 2_554 ?
Ge1 O5 K2 Ge2 141.22(9) . . . 2_554 ?
K1 O5 K2 Ge2 65.29(6) . . . 2_554 ?
Ge2 O5 K2 Ge1 148.2(2) . . . . ?
K1 O5 K2 Ge1 -75.94(11) . . . . ?
Ge2 O5 K2 K1 -135.83(14) . . . . ?
Ge1 O5 K2 K1 75.94(11) . . . . ?
Ge2 O3 K2 O5 -2.69(9) . . . . ?
K2 O3 K2 O5 85.66(9) 2 . . . ?
K2 O3 K2 O5 -89.29(9) 2_554 . . . ?
K1 O3 K2 O5 159.27(11) 2 . . . ?
Ge2 O3 K2 O4 -145.10(9) . . . 2 ?
K2 O3 K2 O4 -56.75(8) 2 . . 2 ?
K2 O3 K2 O4 128.30(8) 2_554 . . 2 ?
K1 O3 K2 O4 16.86(9) 2 . . 2 ?
Ge2 O3 K2 O4 21.7(2) . . . 6_556 ?
K2 O3 K2 O4 110.09(18) 2 . . 6_556 ?
K2 O3 K2 O4 -64.87(19) 2_554 . . 6_556 ?
K1 O3 K2 O4 -176.31(15) 2 . . 6_556 ?
Ge2 O3 K2 O6 142.70(9) . . . 2_554 ?
K2 O3 K2 O6 -128.95(8) 2 . . 2_554 ?
K2 O3 K2 O6 56.10(8) 2_554 . . 2_554 ?
K1 O3 K2 O6 -55.34(9) 2 . . 2_554 ?
Ge2 O3 K2 O3 86.58(10) . . . 2_554 ?
K2 O3 K2 O3 174.93(10) 2 . . 2_554 ?
K2 O3 K2 O3 -0.023(4) 2_554 . . 2_554 ?
K1 O3 K2 O3 -111.47(9) 2 . . 2_554 ?
Ge2 O3 K2 O3 -88.37(10) . . . 2 ?
K2 O3 K2 O3 -0.023(5) 2 . . 2 ?
K2 O3 K2 O3 -174.98(10) 2_554 . . 2 ?
K1 O3 K2 O3 73.58(6) 2 . . 2 ?
Ge2 O3 K2 O2 -18.77(12) . . . . ?
K2 O3 K2 O2 69.58(8) 2 . . . ?
K2 O3 K2 O2 -105.37(8) 2_554 . . . ?
K1 O3 K2 O2 143.18(8) 2 . . . ?
Ge2 O3 K2 Ge2 -119.49(9) . . . 2 ?
K2 O3 K2 Ge2 -31.14(5) 2 . . 2 ?
K2 O3 K2 Ge2 153.91(6) 2_554 . . 2 ?
K1 O3 K2 Ge2 42.46(6) 2 . . 2 ?
Ge2 O3 K2 Ge2 117.53(9) . . . 2_554 ?
K2 O3 K2 Ge2 -154.12(6) 2 . . 2_554 ?
K2 O3 K2 Ge2 30.93(5) 2_554 . . 2_554 ?
K1 O3 K2 Ge2 -80.52(6) 2 . . 2_554 ?
Ge2 O3 K2 Ge1 -18.20(8) . . . . ?
K2 O3 K2 Ge1 70.15(5) 2 . . . ?
K2 O3 K2 Ge1 -104.80(6) 2_554 . . . ?
K1 O3 K2 Ge1 143.75(7) 2 . . . ?
Ge2 O3 K2 K1 31.39(10) . . . . ?
K2 O3 K2 K1 119.74(6) 2 . . . ?
K2 O3 K2 K1 -55.21(6) 2_554 . . . ?
K1 O3 K2 K1 -166.65(6) 2 . . . ?
Ge1 O2 K2 O5 -14.81(10) . . . . ?
Tb1 O2 K2 O5 169.39(16) 6_557 . . . ?
K1 O2 K2 O5 75.59(10) . . . . ?
K1 O2 K2 O5 -98.72(13) 1_556 . . . ?
K2 O2 K2 O5 66.0(2) 8_565 . . . ?
Ge1 O2 K2 O4 121.59(12) . . . 2 ?
Tb1 O2 K2 O4 -54.21(13) 6_557 . . 2 ?
K1 O2 K2 O4 -148.01(8) . . . 2 ?
K1 O2 K2 O4 37.69(14) 1_556 . . 2 ?
K2 O2 K2 O4 -157.58(17) 8_565 . . 2 ?
Ge1 O2 K2 O4 -161.25(16) . . . 6_556 ?
Tb1 O2 K2 O4 22.95(9) 6_557 . . 6_556 ?
K1 O2 K2 O4 -70.85(9) . . . 6_556 ?
K1 O2 K2 O4 114.85(13) 1_556 . . 6_556 ?
K2 O2 K2 O4 -80.4(2) 8_565 . . 6_556 ?
Ge1 O2 K2 O6 -150.37(11) . . . 2_554 ?
Tb1 O2 K2 O6 33.83(19) 6_557 . . 2_554 ?
K1 O2 K2 O6 -59.97(15) . . . 2_554 ?
K1 O2 K2 O6 125.72(12) 1_556 . . 2_554 ?
K2 O2 K2 O6 -69.5(3) 8_565 . . 2_554 ?
Ge1 O2 K2 O3 -94.04(13) . . . 2_554 ?
Tb1 O2 K2 O3 90.16(11) 6_557 . . 2_554 ?
K1 O2 K2 O3 -3.64(9) . . . 2_554 ?
K1 O2 K2 O3 -177.94(10) 1_556 . . 2_554 ?
K2 O2 K2 O3 -13.2(2) 8_565 . . 2_554 ?
Ge1 O2 K2 O3 87.47(13) . . . 2 ?
Tb1 O2 K2 O3 -88.33(11) 6_557 . . 2 ?
K1 O2 K2 O3 177.87(10) . . . 2 ?
K1 O2 K2 O3 3.56(9) 1_556 . . 2 ?
K2 O2 K2 O3 168.3(2) 8_565 . . 2 ?
Ge1 O2 K2 O3 1.20(14) . . . . ?
Tb1 O2 K2 O3 -174.60(10) 6_557 . . . ?
K1 O2 K2 O3 91.60(8) . . . . ?
K1 O2 K2 O3 -82.71(11) 1_556 . . . ?
K2 O2 K2 O3 82.0(2) 8_565 . . . ?
Ge1 O2 K2 Ge2 96.88(12) . . . 2 ?
Tb1 O2 K2 Ge2 -78.92(10) 6_557 . . 2 ?
K1 O2 K2 Ge2 -172.72(6) . . . 2 ?
K1 O2 K2 Ge2 12.97(11) 1_556 . . 2 ?
K2 O2 K2 Ge2 177.71(18) 8_565 . . 2 ?
Ge1 O2 K2 Ge2 -107.07(12) . . . 2_554 ?
Tb1 O2 K2 Ge2 77.13(13) 6_557 . . 2_554 ?
K1 O2 K2 Ge2 -16.67(12) . . . 2_554 ?
K1 O2 K2 Ge2 169.03(6) 1_556 . . 2_554 ?
K2 O2 K2 Ge2 -26.2(3) 8_565 . . 2_554 ?
Tb1 O2 K2 Ge1 -175.8(2) 6_557 . . . ?
K1 O2 K2 Ge1 90.40(13) . . . . ?
K1 O2 K2 Ge1 -83.91(14) 1_556 . . . ?
K2 O2 K2 Ge1 80.8(2) 8_565 . . . ?
Ge1 O2 K2 K1 -90.40(13) . . . . ?
Tb1 O2 K2 K1 93.80(12) 6_557 . . . ?
K1 O2 K2 K1 -174.31(15) 1_556 . . . ?
K2 O2 K2 K1 -9.57(15) 8_565 . . . ?
O2 Ge1 K2 O5 153.36(18) . . . . ?
O1 Ge1 K2 O5 -97.36(17) . . . . ?
O5 Ge1 K2 O5 63.54(16) 8_565 . . . ?
K1 Ge1 K2 O5 -146.63(12) 1_556 . . . ?
K1 Ge1 K2 O5 85.36(12) . . . . ?
K2 Ge1 K2 O5 116.15(12) 8_565 . . . ?
O2 Ge1 K2 O4 -75.54(16) . . . 2 ?
O1 Ge1 K2 O4 33.75(15) . . . 2 ?
O5 Ge1 K2 O4 131.11(15) . . . 2 ?
O5 Ge1 K2 O4 -165.36(13) 8_565 . . 2 ?
K1 Ge1 K2 O4 -15.52(8) 1_556 . . 2 ?
K1 Ge1 K2 O4 -143.54(8) . . . 2 ?
K2 Ge1 K2 O4 -112.75(8) 8_565 . . 2 ?
O2 Ge1 K2 O4 16.14(14) . . . 6_556 ?
O1 Ge1 K2 O4 125.42(13) . . . 6_556 ?
O5 Ge1 K2 O4 -137.22(13) . . . 6_556 ?
O5 Ge1 K2 O4 -73.69(12) 8_565 . . 6_556 ?
K1 Ge1 K2 O4 76.15(6) 1_556 . . 6_556 ?
K1 Ge1 K2 O4 -51.87(6) . . . 6_556 ?
K2 Ge1 K2 O4 -21.07(7) 8_565 . . 6_556 ?
O2 Ge1 K2 O6 68.5(2) . . . 2_554 ?
O1 Ge1 K2 O6 177.8(2) . . . 2_554 ?
O5 Ge1 K2 O6 -84.8(2) . . . 2_554 ?
O5 Ge1 K2 O6 -21.3(2) 8_565 . . 2_554 ?
K1 Ge1 K2 O6 128.53(18) 1_556 . . 2_554 ?
K1 Ge1 K2 O6 0.51(18) . . . 2_554 ?
K2 Ge1 K2 O6 31.3(2) 8_565 . . 2_554 ?
O2 Ge1 K2 O3 93.27(15) . . . 2_554 ?
O1 Ge1 K2 O3 -157.45(13) . . . 2_554 ?
O5 Ge1 K2 O3 -60.09(13) . . . 2_554 ?
O5 Ge1 K2 O3 3.45(13) 8_565 . . 2_554 ?
K1 Ge1 K2 O3 153.28(6) 1_556 . . 2_554 ?
K1 Ge1 K2 O3 25.27(6) . . . 2_554 ?
K2 Ge1 K2 O3 56.06(7) 8_565 . . 2_554 ?
O2 Ge1 K2 O3 -82.62(14) . . . 2 ?
O1 Ge1 K2 O3 26.66(14) . . . 2 ?
O5 Ge1 K2 O3 124.02(14) . . . 2 ?
O5 Ge1 K2 O3 -172.44(12) 8_565 . . 2 ?
K1 Ge1 K2 O3 -22.60(6) 1_556 . . 2 ?
K1 Ge1 K2 O3 -150.62(6) . . . 2 ?
K2 Ge1 K2 O3 -119.83(6) 8_565 . . 2 ?
O2 Ge1 K2 O3 -178.80(14) . . . . ?
O1 Ge1 K2 O3 -69.51(13) . . . . ?
O5 Ge1 K2 O3 27.85(13) . . . . ?
O5 Ge1 K2 O3 91.38(12) 8_565 . . . ?
K1 Ge1 K2 O3 -118.78(5) 1_556 . . . ?
K1 Ge1 K2 O3 113.20(5) . . . . ?
K2 Ge1 K2 O3 144.00(5) 8_565 . . . ?
O1 Ge1 K2 O2 109.28(18) . . . . ?
O5 Ge1 K2 O2 -153.36(18) . . . . ?
O5 Ge1 K2 O2 -89.82(17) 8_565 . . . ?
K1 Ge1 K2 O2 60.02(13) 1_556 . . . ?
K1 Ge1 K2 O2 -68.00(14) . . . . ?
K2 Ge1 K2 O2 -37.21(14) 8_565 . . . ?
O2 Ge1 K2 Ge2 -88.39(14) . . . 2 ?
O1 Ge1 K2 Ge2 20.89(13) . . . 2 ?
O5 Ge1 K2 Ge2 118.25(13) . . . 2 ?
O5 Ge1 K2 Ge2 -178.22(11) 8_565 . . 2 ?
K1 Ge1 K2 Ge2 -28.38(3) 1_556 . . 2 ?
K1 Ge1 K2 Ge2 -156.40(4) . . . 2 ?
K2 Ge1 K2 Ge2 -125.60(2) 8_565 . . 2 ?
O2 Ge1 K2 Ge2 100.42(14) . . . 2_554 ?
O1 Ge1 K2 Ge2 -150.30(13) . . . 2_554 ?
O5 Ge1 K2 Ge2 -52.94(13) . . . 2_554 ?
O5 Ge1 K2 Ge2 10.60(13) 8_565 . . 2_554 ?
K1 Ge1 K2 Ge2 160.44(5) 1_556 . . 2_554 ?
K1 Ge1 K2 Ge2 32.42(5) . . . 2_554 ?
K2 Ge1 K2 Ge2 63.21(7) 8_565 . . 2_554 ?
O2 Ge1 K2 K1 68.00(14) . . . . ?
O1 Ge1 K2 K1 177.28(12) . . . . ?
O5 Ge1 K2 K1 -85.36(12) . . . . ?
O5 Ge1 K2 K1 -21.82(11) 8_565 . . . ?
K1 Ge1 K2 K1 128.02(4) 1_556 . . . ?
K2 Ge1 K2 K1 30.79(4) 8_565 . . . ?
O1 K1 K2 O5 55.42(10) 1_554 . . . ?
O2 K1 K2 O5 -67.07(11) . . . . ?
O6 K1 K2 O5 164.84(9) 6_556 . . . ?
O6 K1 K2 O5 -160.67(10) 3_455 . . . ?
O2 K1 K2 O5 119.33(11) 1_554 . . . ?
O5 K1 K2 O5 -23.53(5) 8_565 . . . ?
O3 K1 K2 O5 117.21(9) 2_554 . . . ?
O3 K1 K2 O5 -57.4(3) 7_665 . . . ?
O4 K1 K2 O5 -143.36(9) 6_556 . . . ?
O4 K1 K2 O5 -110.11(8) 3_455 . . . ?
Ge1 K1 K2 O5 85.04(7) 1_554 . . . ?
O1 K1 K2 O4 -163.45(13) 1_554 . . 2 ?
O2 K1 K2 O4 74.05(15) . . . 2 ?
O6 K1 K2 O4 -54.03(13) 6_556 . . 2 ?
O6 K1 K2 O4 -19.54(15) 3_455 . . 2 ?
O2 K1 K2 O4 -99.54(15) 1_554 . . 2 ?
O5 K1 K2 O4 117.59(13) 8_565 . . 2 ?
O5 K1 K2 O4 141.13(14) . . . 2 ?
O3 K1 K2 O4 -101.67(14) 2_554 . . 2 ?
O3 K1 K2 O4 83.7(3) 7_665 . . 2 ?
O4 K1 K2 O4 -2.23(17) 6_556 . . 2 ?
O4 K1 K2 O4 31.02(15) 3_455 . . 2 ?
Ge1 K1 K2 O4 -133.84(12) 1_554 . . 2 ?
O1 K1 K2 O4 -161.22(10) 1_554 . . 6_556 ?
O2 K1 K2 O4 76.28(10) . . . 6_556 ?
O6 K1 K2 O4 -51.80(8) 6_556 . . 6_556 ?
O6 K1 K2 O4 -17.31(10) 3_455 . . 6_556 ?
O2 K1 K2 O4 -97.31(11) 1_554 . . 6_556 ?
O5 K1 K2 O4 119.82(8) 8_565 . . 6_556 ?
O5 K1 K2 O4 143.36(9) . . . 6_556 ?
O3 K1 K2 O4 -99.44(9) 2_554 . . 6_556 ?
O3 K1 K2 O4 85.9(3) 7_665 . . 6_556 ?
O4 K1 K2 O4 33.25(6) 3_455 . . 6_556 ?
Ge1 K1 K2 O4 -131.60(7) 1_554 . . 6_556 ?
O1 K1 K2 O6 -91.69(9) 1_554 . . 2_554 ?
O2 K1 K2 O6 145.82(10) . . . 2_554 ?
O6 K1 K2 O6 17.73(10) 6_556 . . 2_554 ?
O6 K1 K2 O6 52.22(11) 3_455 . . 2_554 ?
O2 K1 K2 O6 -27.78(11) 1_554 . . 2_554 ?
O5 K1 K2 O6 -170.64(7) 8_565 . . 2_554 ?
O5 K1 K2 O6 -147.11(9) . . . 2_554 ?
O3 K1 K2 O6 -29.90(8) 2_554 . . 2_554 ?
O3 K1 K2 O6 155.5(3) 7_665 . . 2_554 ?
O4 K1 K2 O6 69.53(8) 6_556 . . 2_554 ?
O4 K1 K2 O6 102.78(8) 3_455 . . 2_554 ?
Ge1 K1 K2 O6 -62.07(7) 1_554 . . 2_554 ?
O1 K1 K2 O3 -61.79(9) 1_554 . . 2_554 ?
O2 K1 K2 O3 175.72(11) . . . 2_554 ?
O6 K1 K2 O3 47.63(8) 6_556 . . 2_554 ?
O6 K1 K2 O3 82.13(10) 3_455 . . 2_554 ?
O2 K1 K2 O3 2.13(11) 1_554 . . 2_554 ?
O5 K1 K2 O3 -140.74(8) 8_565 . . 2_554 ?
O5 K1 K2 O3 -117.21(9) . . . 2_554 ?
O3 K1 K2 O3 -174.6(3) 7_665 . . 2_554 ?
O4 K1 K2 O3 99.44(9) 6_556 . . 2_554 ?
O4 K1 K2 O3 132.69(8) 3_455 . . 2_554 ?
Ge1 K1 K2 O3 -32.17(7) 1_554 . . 2_554 ?
O1 K1 K2 O3 120.20(10) 1_554 . . 2 ?
O2 K1 K2 O3 -2.29(11) . . . 2 ?
O6 K1 K2 O3 -130.38(8) 6_556 . . 2 ?
O6 K1 K2 O3 -95.88(10) 3_455 . . 2 ?
O2 K1 K2 O3 -175.88(10) 1_554 . . 2 ?
O5 K1 K2 O3 41.25(9) 8_565 . . 2 ?
O5 K1 K2 O3 64.78(9) . . . 2 ?
O3 K1 K2 O3 -178.01(13) 2_554 . . 2 ?
O3 K1 K2 O3 7.4(3) 7_665 . . 2 ?
O4 K1 K2 O3 -78.57(9) 6_556 . . 2 ?
O4 K1 K2 O3 -45.32(9) 3_455 . . 2 ?
Ge1 K1 K2 O3 149.82(7) 1_554 . . 2 ?
O1 K1 K2 O3 23.37(9) 1_554 . . . ?
O2 K1 K2 O3 -99.12(10) . . . . ?
O6 K1 K2 O3 132.79(7) 6_556 . . . ?
O6 K1 K2 O3 167.28(9) 3_455 . . . ?
O2 K1 K2 O3 87.29(10) 1_554 . . . ?
O5 K1 K2 O3 -55.58(7) 8_565 . . . ?
O5 K1 K2 O3 -32.05(8) . . . . ?
O3 K1 K2 O3 85.16(8) 2_554 . . . ?
O3 K1 K2 O3 -89.5(3) 7_665 . . . ?
O4 K1 K2 O3 -175.41(8) 6_556 . . . ?
O4 K1 K2 O3 -142.15(7) 3_455 . . . ?
Ge1 K1 K2 O3 52.99(6) 1_554 . . . ?
O1 K1 K2 O2 122.49(11) 1_554 . . . ?
O6 K1 K2 O2 -128.09(10) 6_556 . . . ?
O6 K1 K2 O2 -93.60(11) 3_455 . . . ?
O2 K1 K2 O2 -173.59(17) 1_554 . . . ?
O5 K1 K2 O2 43.54(9) 8_565 . . . ?
O5 K1 K2 O2 67.07(11) . . . . ?
O3 K1 K2 O2 -175.72(11) 2_554 . . . ?
O3 K1 K2 O2 9.7(3) 7_665 . . . ?
O4 K1 K2 O2 -76.28(10) 6_556 . . . ?
O4 K1 K2 O2 -43.03(9) 3_455 . . . ?
Ge1 K1 K2 O2 152.11(10) 1_554 . . . ?
O1 K1 K2 Ge2 136.20(9) 1_554 . . 2 ?
O2 K1 K2 Ge2 13.70(11) . . . 2 ?
O6 K1 K2 Ge2 -114.38(8) 6_556 . . 2 ?
O6 K1 K2 Ge2 -79.89(10) 3_455 . . 2 ?
O2 K1 K2 Ge2 -159.89(9) 1_554 . . 2 ?
O5 K1 K2 Ge2 57.24(9) 8_565 . . 2 ?
O5 K1 K2 Ge2 80.78(9) . . . 2 ?
O3 K1 K2 Ge2 -162.02(9) 2_554 . . 2 ?
O3 K1 K2 Ge2 23.4(3) 7_665 . . 2 ?
O4 K1 K2 Ge2 -62.58(9) 6_556 . . 2 ?
O4 K1 K2 Ge2 -29.33(9) 3_455 . . 2 ?
Ge1 K1 K2 Ge2 165.81(5) 1_554 . . 2 ?
O1 K1 K2 Ge2 -69.56(7) 1_554 . . 2_554 ?
O2 K1 K2 Ge2 167.94(9) . . . 2_554 ?
O6 K1 K2 Ge2 39.86(5) 6_556 . . 2_554 ?
O6 K1 K2 Ge2 74.35(8) 3_455 . . 2_554 ?
O2 K1 K2 Ge2 -5.65(9) 1_554 . . 2_554 ?
O5 K1 K2 Ge2 -148.52(5) 8_565 . . 2_554 ?
O5 K1 K2 Ge2 -124.98(7) . . . 2_554 ?
O3 K1 K2 Ge2 -7.78(6) 2_554 . . 2_554 ?
O3 K1 K2 Ge2 177.6(3) 7_665 . . 2_554 ?
O4 K1 K2 Ge2 91.66(6) 6_556 . . 2_554 ?
O4 K1 K2 Ge2 124.91(5) 3_455 . . 2_554 ?
Ge1 K1 K2 Ge2 -39.95(4) 1_554 . . 2_554 ?
O1 K1 K2 Ge1 88.13(8) 1_554 . . . ?
O2 K1 K2 Ge1 -34.36(8) . . . . ?
O6 K1 K2 Ge1 -162.45(6) 6_556 . . . ?
O6 K1 K2 Ge1 -127.95(8) 3_455 . . . ?
O2 K1 K2 Ge1 152.05(10) 1_554 . . . ?
O5 K1 K2 Ge1 9.18(5) 8_565 . . . ?
O5 K1 K2 Ge1 32.71(6) . . . . ?
O3 K1 K2 Ge1 149.92(7) 2_554 . . . ?
O3 K1 K2 Ge1 -24.7(3) 7_665 . . . ?
O4 K1 K2 Ge1 -110.64(6) 6_556 . . . ?
O4 K1 K2 Ge1 -77.39(5) 3_455 . . . ?
Ge1 K1 K2 Ge1 117.75(5) 1_554 . . . ?

_diffrn_measured_fraction_theta_max 1.000
_diffrn_reflns_theta_full        26.35
_diffrn_measured_fraction_theta_full 1.000
_refine_diff_density_max         0.945
_refine_diff_density_min         -1.429
_refine_diff_density_rms         0.196
_database_code_depnum_ccdc_archive 'CCDC 995426'
